# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2022

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_iw2a_sq
_database_code_depnum_ccdc_archive 'CCDC 2075364'
loop_
_audit_author_name
_audit_author_address
'Mark Baranov'
;Ben Gurion University of the Negev
Israel
;
_audit_update_record             
;
2021-04-05 deposited with the CCDC.	2022-01-03 downloaded from the CCDC.
;
# start Validation Reply Form
_vrf_PLAT306_iw2a_sq             
;
PROBLEM: Isolated Oxygen Atom (H-atoms Missing ?) ....... Check
RESPONSE: These are solvent water molecules, 
it was not possible to assign hydrogen atoms
as the structure contains many heavy atoms
;
# end Validation Reply Form
_audit_creation_date             2021-04-05
_audit_creation_method           
;
Olex2 1.3
(compiled 2020.11.12 svn.r5f609507 for OlexSys, GUI svn.r6226)
;
_shelx_SHELXL_version_number     2018/3
_audit_contact_author_address    ?
_audit_contact_author_email      ?
_audit_contact_author_phone      ?
_publ_contact_author_id_orcid    ?
_publ_section_references         
;
Dolomanov, O.V., Bourhis, L.J., Gildea, R.J, Howard, J.A.K. & Puschmann, H.
 (2009), J. Appl. Cryst. 42, 339-341.

Sheldrick, G.M. (2015). Acta Cryst. C71, 3-8.
;
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         
'Fe8 Li18 Nb48 O162, 52(O), Li8 O2, 1.571(Li14)'
_chemical_formula_sum            'Fe8 Li48 Nb48 O216'
_chemical_formula_weight         8695.60
_chemical_melting_point          ?
_chemical_oxdiff_formula         Nb12Fe1O50Li2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Fe Fe -1.1336 3.1974 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Li Li 0.0008 0.0003 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nb Nb -0.1121 2.4826 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0492 0.0322 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      orthorhombic
_space_group_IT_number           56
_space_group_name_H-M_alt        'P c c n'
_space_group_name_Hall           '-P 2ab 2ac'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y+1/2, z'
'-x, y+1/2, -z+1/2'
'x+1/2, -y, -z+1/2'
'-x, -y, -z'
'x-1/2, y-1/2, -z'
'x, -y-1/2, z-1/2'
'-x-1/2, y, z-1/2'

_cell_length_a                   22.5729(6)
_cell_length_b                   32.4190(3)
_cell_length_c                   43.4373(5)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     31787.0(10)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    35767
_cell_measurement_temperature    100.01(10)
_cell_measurement_theta_max      76.4080
_cell_measurement_theta_min      4.0960
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    17.118
_exptl_absorpt_correction_T_max  1.000
_exptl_absorpt_correction_T_min  0.366
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details   
;
CrysAlisPro 1.171.39.46 (Rigaku Oxford Diffraction, 2018)
Numerical absorption correction based on gaussian integration over
			a multifaceted crystal model
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            yellow
_exptl_crystal_colour_primary    yellow
_exptl_crystal_density_diffrn    1.817
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       plate
_exptl_crystal_F_000             16192
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
-4 -3 27 0.1922
10 -16 -1 0.0198
-11 -14 -1 0.0074
0 1 -28 0.3768
11 14 0 0.0393
2 1 28 0.1925
-9 16 -1 0.0217

_exptl_crystal_size_max          0.574
_exptl_crystal_size_mid          0.058
_exptl_crystal_size_min          0.053
loop_
_exptl_oxdiff_crystal_face_indexfrac_h
_exptl_oxdiff_crystal_face_indexfrac_k
_exptl_oxdiff_crystal_face_indexfrac_l
_exptl_oxdiff_crystal_face_x
_exptl_oxdiff_crystal_face_y
_exptl_oxdiff_crystal_face_z
-3.8237 -2.7675 26.9670 -0.0021 0.1217 0.9926
9.6938 -15.7255 -1.4172 0.0007 -1.0000 0.0000
-10.9891 -13.9121 -1.2045 -0.9704 -0.0005 0.2416
-0.0155 1.3376 -28.1384 -0.2427 -0.0012 -0.9701
10.9829 13.9495 0.2665 0.9618 0.0004 -0.2737
2.0321 0.9817 28.0187 0.4104 -0.0077 0.9167
-8.9739 15.9735 -0.8860 0.0193 0.9722 -0.0897

_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0789
_diffrn_reflns_av_unetI/netI     0.0526
_diffrn_reflns_Laue_measured_fraction_full 0.986
_diffrn_reflns_Laue_measured_fraction_max 0.980
_diffrn_reflns_limit_h_max       24
_diffrn_reflns_limit_h_min       -28
_diffrn_reflns_limit_k_max       33
_diffrn_reflns_limit_k_min       -39
_diffrn_reflns_limit_l_max       53
_diffrn_reflns_limit_l_min       -39
_diffrn_reflns_number            128352
_diffrn_reflns_point_group_measured_fraction_full 0.986
_diffrn_reflns_point_group_measured_fraction_max 0.980
_diffrn_reflns_theta_full        67.684
_diffrn_reflns_theta_max         74.503
_diffrn_reflns_theta_min         3.508
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      100.01(10)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.986
_diffrn_measured_fraction_theta_max 0.980
_diffrn_measurement_details      
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
#--------------------------------------------------------------------------
  1  ω     19.00 130.00   0.30   10.00    --   45.10  57.00 150.00  370
  2  ω      5.00 118.10   0.30   10.00    --   45.10  57.00   0.00  377
  3  ω     33.00 128.10   0.30   10.00    --   45.10  57.00  60.00  317
  4  ω     -1.00  30.20   0.30   10.00    --   45.10 -77.00-120.00  104
  5  ω     57.00  85.20   0.30   10.00    --   45.10 -77.00-120.00   94
  6  ω     99.00 133.20   0.30   60.00    --  114.00 -77.00  30.00  114
  7  ω     54.00 119.10   0.30   60.00    --  114.00 -77.00-120.00  217
  8  ω     25.00 157.00   0.30   60.00    --  114.00 -77.00   0.00  440
  9  ω     80.00 107.00   0.30   60.00    --  114.00 -77.00 -60.00   90
 10  ω     25.00 127.00   0.30   60.00    --  114.00 -50.00 120.00  340
 11  ω     33.00  75.00   0.30   60.00    --  114.00 -77.00  30.00  140
 12  ω     38.00 123.20   0.30   60.00    --  114.00 -38.00 120.00  284
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'XtaLAB AFC12 (RINC): Kappa dual home/near'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_type       
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      0.0496558000
_diffrn_orient_matrix_UB_12      0.0296620000
_diffrn_orient_matrix_UB_13      0.0100069000
_diffrn_orient_matrix_UB_21      -0.0451900000
_diffrn_orient_matrix_UB_22      0.0355757000
_diffrn_orient_matrix_UB_23      0.0017573000
_diffrn_orient_matrix_UB_31      -0.0122604000
_diffrn_orient_matrix_UB_32      -0.0106201000
_diffrn_orient_matrix_UB_33      0.0339782000
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.54184
_diffrn_source                   'micro-focus sealed X-ray tube'
_diffrn_source_type              'Rigaku (Cu) X-ray Source'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                24542
_reflns_number_total             31875
_reflns_odcompleteness_completeness 97.89
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     74.33
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_computing_data_collection       'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_computing_data_reduction        'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_refine_diff_density_max         1.935
_refine_diff_density_min         -1.659
_refine_diff_density_rms         0.236
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.086
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1449
_refine_ls_number_reflns         31875
_refine_ls_number_restraints     12
_refine_ls_R_factor_all          0.0895
_refine_ls_R_factor_gt           0.0767
_refine_ls_restrained_S_all      1.086
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.1707P)²+31.9223P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2338
_refine_ls_wR_factor_ref         0.2479
_refine_special_details          SQUEEZE
_olex2_refinement_description    
;
1. Uiso/Uaniso restraints and constraints
Uanis(Li24) \\sim Ueq: with sigma of 0.001 and sigma for terminal atoms of 0.002
Uanis(Li23) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(O30) = Uanis(Nb23) = Uanis(Nb25)
2. Others
 Sof(Nb3)=Sof(Nb25)=1-FVAR(1)
 Sof(Nb11)=Sof(Nb23)=FVAR(1)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Nb1 Nb 0.87132(4) 0.56532(2) 0.63824(2) 0.04773(17) Uani 1 1 d . . . . .
Nb4 Nb 0.65666(4) 0.59841(2) 0.75751(2) 0.05014(18) Uani 1 1 d . . . . .
Nb6 Nb 0.70112(4) 0.68668(2) 0.78802(2) 0.04949(18) Uani 1 1 d . . . . .
Nb8 Nb 0.80109(4) 0.61822(2) 0.75922(2) 0.05088(18) Uani 1 1 d . . . . .
Nb10 Nb 0.79387(4) 0.63340(2) 0.83738(2) 0.05208(18) Uani 1 1 d . . . . .
Nb12 Nb 0.65917(4) 0.71497(2) 0.52041(2) 0.05198(18) Uani 1 1 d . . . . .
Nb14 Nb 0.74716(4) 0.54604(2) 0.80551(2) 0.05300(18) Uani 1 1 d . . . . .
Nb16 Nb 0.82581(4) 0.59935(2) 0.56859(2) 0.05486(19) Uani 1 1 d . . . . .
Nb18 Nb 0.55975(4) 0.78415(2) 0.54950(2) 0.05493(19) Uani 1 1 d . . . . .
Nb20 Nb 0.64868(4) 0.61286(2) 0.83391(2) 0.05346(19) Uani 1 1 d . . . . .
Nb22 Nb 0.73882(4) 0.53856(2) 0.61028(2) 0.05514(19) Uani 1 1 d . . . . .
Nb24 Nb 0.57889(4) 0.77736(2) 0.47154(2) 0.05349(19) Uani 1 1 d . . . . .
Nb26 Nb 0.48582(4) 0.83619(2) 0.66835(2) 0.05670(19) Uani 1 1 d . . . . .
Nb13 Nb 0.93661(4) 0.52711(3) 0.57246(2) 0.05637(19) Uani 1 1 d . . . . .
Nb7 Nb 0.84728(4) 0.46840(2) 0.61498(2) 0.0579(2) Uani 1 1 d . . . . .
Nb15 Nb 0.53434(4) 0.80376(2) 0.73805(2) 0.0622(2) Uani 1 1 d . . . . .
Nb2 Nb 0.53334(4) 0.68317(3) 0.55245(2) 0.0608(2) Uani 1 1 d . . . . .
Nb17 Nb 0.43036(4) 0.88078(3) 0.73385(2) 0.0624(2) Uani 1 1 d . . . . .
Nb9 Nb 0.55189(4) 0.67626(3) 0.47618(2) 0.0611(2) Uani 1 1 d . . . . .
Nb19 Nb 0.80241(5) 0.50239(3) 0.54611(2) 0.0631(2) Uani 1 1 d . . . . .
Nb5 Nb 0.45499(4) 0.74380(3) 0.50495(2) 0.0651(2) Uani 1 1 d . . . . .
Nb21 Nb 0.34663(5) 0.81894(3) 0.69023(3) 0.0781(3) Uani 1 1 d . . . . .
Nb11 Nb 0.44696(10) 0.74445(6) 0.69860(6) 0.0601(4) Uani 0.732(5) 1 d . . P A 1
Nb23 Nb 0.39446(8) 0.78961(6) 0.76193(6) 0.0651(4) Uani 0.732(5) 1 d . . P A 1
Fe1 Fe 0.93635(6) 0.60596(4) 0.71216(3) 0.0442(3) Uani 1 1 d . . . . .
Fe4 Fe 0.82018(6) 0.68848(4) 0.51619(3) 0.0460(3) Uani 1 1 d . . . . .
Fe2 Fe 0.65994(7) 0.79758(4) 0.79126(3) 0.0494(3) Uani 1 1 d . . . . .
Fe3 Fe 0.54435(7) 0.88035(4) 0.59452(3) 0.0487(3) Uani 1 1 d . . . . .
O26 O 0.4787(3) 0.88965(18) 0.69383(14) 0.0541(15) Uani 1 1 d . . . . .
O54 O 0.7266(3) 0.61806(16) 0.79670(13) 0.0494(14) Uani 1 1 d . . . . .
O43 O 0.7308(3) 0.80923(18) 0.82028(14) 0.0538(15) Uani 1 1 d . . . . .
O51 O 0.7746(3) 0.67888(18) 0.76101(13) 0.0524(14) Uani 1 1 d . . . . .
O64 O 0.8638(3) 0.61539(19) 0.60958(15) 0.0538(14) Uani 1 1 d . . . . .
O53 O 0.7326(3) 0.60533(18) 0.73402(14) 0.0526(14) Uani 1 1 d . . . . .
O63 O 0.7862(3) 0.56601(18) 0.64453(14) 0.0512(14) Uani 1 1 d . . . . .
O3 O 0.8379(3) 0.73853(19) 0.48785(14) 0.0527(14) Uani 1 1 d . . . . .
O50 O 0.6066(3) 0.59946(19) 0.79538(13) 0.0539(15) Uani 1 1 d . . . . .
O37 O 0.5583(3) 0.83114(18) 0.69718(16) 0.0549(15) Uani 1 1 d . . . . .
O4 O 0.7374(3) 0.7039(2) 0.52337(16) 0.0586(16) Uani 1 1 d . . . . .
O73 O 0.8764(3) 0.50748(19) 0.64735(13) 0.0534(14) Uani 1 1 d . . . . .
O75 O 0.6818(3) 0.55698(19) 0.83445(14) 0.0588(16) Uani 1 1 d . . . . .
O60 O 0.9855(3) 0.63519(19) 0.74704(15) 0.0562(15) Uani 1 1 d . . . . .
O8 O 0.6476(3) 0.76588(19) 0.54751(13) 0.0512(14) Uani 1 1 d . . . . .
O71 O 0.9485(3) 0.56023(19) 0.61281(14) 0.0509(13) Uani 1 1 d . . . . .
O58 O 0.8094(3) 0.56280(19) 0.77434(15) 0.0539(14) Uani 1 1 d . . . . .
O41 O 0.6556(3) 0.86130(18) 0.79811(15) 0.0537(14) Uani 1 1 d . . . . .
O47 O 0.6518(3) 0.65985(19) 0.75739(14) 0.0537(14) Uani 1 1 d . . . . .
O80 O 0.6883(3) 0.54455(18) 0.77141(14) 0.0529(14) Uani 1 1 d . . . . .
O59 O 0.8602(3) 0.6196(2) 0.73080(16) 0.0594(16) Uani 1 1 d . . . . .
O6 O 0.6237(3) 0.6810(2) 0.55144(15) 0.0593(16) Uani 1 1 d . . . . .
O45 O 0.6470(3) 0.6721(2) 0.82065(14) 0.0540(14) Uani 1 1 d . . . . .
O68 O 0.9142(3) 0.5873(2) 0.55972(14) 0.0563(15) Uani 1 1 d . . . . .
O56 O 0.8013(3) 0.5745(2) 0.83536(16) 0.0596(16) Uani 1 1 d . . . . .
O49 O 0.7198(3) 0.63063(18) 0.85940(14) 0.0547(15) Uani 1 1 d . . . . .
O5 O 0.6375(3) 0.6765(2) 0.48828(16) 0.0611(16) Uani 1 1 d . . . . .
O14 O 0.5868(3) 0.81423(19) 0.50964(14) 0.0534(15) Uani 1 1 d . . . . .
O66 O 0.7503(3) 0.5926(2) 0.58808(15) 0.0570(15) Uani 1 1 d . . . . .
O13 O 0.4945(4) 0.7822(2) 0.47417(17) 0.0683(19) Uani 1 1 d . . . . .
O34 O 0.9274(3) 0.47669(19) 0.59610(15) 0.0578(15) Uani 1 1 d . . . . .
O72 O 0.7655(3) 0.4853(2) 0.62606(16) 0.0624(17) Uani 1 1 d . . . . .
O16 O 0.5747(3) 0.7251(2) 0.44958(15) 0.0600(16) Uani 1 1 d . . . . .
O44 O 0.6838(3) 0.73990(19) 0.78360(15) 0.0592(16) Uani 1 1 d . . . . .
O10 O 0.5585(3) 0.7313(2) 0.51269(15) 0.0557(15) Uani 1 1 d . . . . .
O52 O 0.6040(3) 0.5844(2) 0.72829(15) 0.0617(16) Uani 1 1 d . . . . .
O11 O 0.4791(3) 0.7869(2) 0.53596(18) 0.0668(18) Uani 1 1 d . . . . .
O62 O 0.8999(3) 0.58772(18) 0.67350(13) 0.0514(14) Uani 1 1 d . . . . .
O77 O 0.8905(3) 0.5064(2) 0.53899(14) 0.0599(16) Uani 1 1 d . . . . .
O40 O 0.6049(3) 0.7980(2) 0.7568(2) 0.0702(19) Uani 1 1 d . . . . .
O33 O 0.4436(3) 0.8135(2) 0.71437(17) 0.0607(16) Uani 1 1 d . . . . .
O70 O 0.8385(3) 0.53614(18) 0.59214(14) 0.0517(14) Uani 1 1 d . . . . .
O61 O 0.9471(4) 0.5530(2) 0.73037(16) 0.0653(18) Uani 1 1 d . . . . .
O23 O 0.4036(3) 0.8400(2) 0.65822(19) 0.0690(19) Uani 1 1 d . . . . .
O1 O 0.8188(3) 0.6484(2) 0.55016(18) 0.0671(18) Uani 1 1 d . . . . .
O67 O 0.8035(3) 0.5629(2) 0.53519(15) 0.0615(16) Uani 1 1 d . . . . .
O9 O 0.5430(4) 0.7372(2) 0.57531(16) 0.0651(18) Uani 1 1 d . . . . .
O69 O 0.7294(3) 0.5131(2) 0.56985(16) 0.0638(17) Uani 1 1 d . . . . .
O48 O 0.5913(4) 0.6110(2) 0.86188(17) 0.0704(19) Uani 1 1 d . . . . .
O46 O 0.4555(3) 0.7046(2) 0.53933(18) 0.0681(19) Uani 1 1 d . . . . .
O76 O 1.0101(4) 0.5244(3) 0.55841(17) 0.072(2) Uani 1 1 d . . . . .
O55 O 0.8466(4) 0.6480(2) 0.86590(17) 0.0676(19) Uani 1 1 d . . . . .
O17 O 0.4710(4) 0.6980(2) 0.47611(18) 0.072(2) Uani 1 1 d . . . . .
O39 O 0.5250(3) 0.7516(2) 0.7178(2) 0.075(2) Uani 1 1 d . . . . .
O65 O 0.6646(4) 0.5421(3) 0.62467(17) 0.073(2) Uani 1 1 d . . . . .
O22 O 0.5200(3) 0.8564(2) 0.63379(15) 0.0577(15) Uani 1 1 d . . . . .
O20 O 0.5620(4) 0.8267(2) 0.57631(17) 0.0675(18) Uani 1 1 d . . . . .
O57 O 0.7611(4) 0.4935(2) 0.81161(19) 0.0690(19) Uani 1 1 d . . . . .
O79 O 0.8179(4) 0.4550(2) 0.57396(16) 0.0660(18) Uani 1 1 d . . . . .
O25 O 0.3593(3) 0.8743(2) 0.7095(2) 0.076(2) Uani 1 1 d . . . . .
O38 O 0.4869(4) 0.7766(2) 0.6620(2) 0.073(2) Uani 1 1 d . . . . .
O19 O 0.5350(4) 0.6482(2) 0.51552(18) 0.0684(19) Uani 1 1 d . . . . .
O31 O 0.4820(4) 0.7891(2) 0.77120(19) 0.075(2) Uani 1 1 d . . . . .
O15 O 0.5999(4) 0.8132(2) 0.44241(16) 0.0672(18) Uani 1 1 d . . . . .
O27 O 0.4277(4) 0.9316(3) 0.74821(18) 0.079(2) Uani 1 1 d . . . . .
O74 O 0.8544(4) 0.4194(2) 0.63312(17) 0.071(2) Uani 1 1 d . . . . .
O21 O 0.4665(4) 0.8890(3) 0.5782(2) 0.081(2) Uani 1 1 d . . . . .
O12 O 0.3795(4) 0.7541(3) 0.4990(2) 0.084(2) Uani 1 1 d . . . . .
O7 O 0.5160(4) 0.6480(3) 0.5819(2) 0.083(2) Uani 1 1 d . . . . .
O29 O 0.3990(4) 0.8490(3) 0.7672(2) 0.082(2) Uani 1 1 d . . . . .
O35 O 0.3729(4) 0.7627(3) 0.6790(3) 0.087(3) Uani 1 1 d . . . . .
O42 O 0.6036(6) 0.7858(3) 0.8223(2) 0.123(5) Uani 1 1 d . . . . .
O32 O 0.4107(4) 0.7374(3) 0.7373(3) 0.096(3) Uani 1 1 d . . . . .
O2 O 0.8093(5) 0.6471(3) 0.4849(2) 0.090(3) Uani 1 1 d . . . . .
O18 O 0.5489(4) 0.6362(3) 0.4482(2) 0.080(2) Uani 1 1 d . . . . .
O28 O 0.3280(4) 0.7986(3) 0.7317(2) 0.093(3) Uani 1 1 d . . . . .
O78 O 0.7749(4) 0.4784(3) 0.51240(17) 0.082(2) Uani 1 1 d . . . . .
O36 O 0.4541(5) 0.6920(3) 0.6835(3) 0.103(3) Uani 1 1 d . . . . .
O24 O 0.2762(4) 0.8236(3) 0.6715(3) 0.102(3) Uani 1 1 d . . . . .
O30 O 0.3586(3) 0.7692(2) 0.79384(17) 0.0651(4) Uani 1 1 d . . . . .
Nb3 Nb 0.4531(2) 0.74180(16) 0.68563(17) 0.0586(12) Uani 0.268(5) 1 d . . P A 2
Nb25 Nb 0.3969(2) 0.77960(17) 0.75047(15) 0.0651(4) Uani 0.268(5) 1 d . . P A 2
O104 O 0.6767(4) 0.4734(2) 0.74129(16) 0.071(2) Uani 1 1 d . . . . .
O81 O 0.3769(4) 0.8997(3) 0.6173(2) 0.086(2) Uani 1 1 d . . . . .
O86 O 0.5175(4) 0.5424(3) 0.8641(2) 0.086(3) Uani 1 1 d . . . . .
O83 O 0.6966(4) 0.6873(2) 0.90407(15) 0.0666(19) Uani 1 1 d . . . . .
O82 O 0.5792(4) 0.5089(3) 0.79806(19) 0.078(2) Uani 1 1 d . . . . .
O85 O 0.4240(4) 0.7620(5) 0.6035(3) 0.141(6) Uani 1 1 d . . . . .
O98 O 0.750000 0.750000 0.8609(2) 0.059(2) Uani 1 2 d S T P . .
O87 O 0.6246(4) 0.5266(3) 0.68335(18) 0.082(2) Uani 1 1 d . . . . .
O109 O 1.0354(3) 0.5477(2) 0.65447(17) 0.0640(17) Uani 1 1 d . . . . .
O89 O 0.6610(5) 0.4459(3) 0.8198(3) 0.112(4) Uani 1 1 d . . . . .
O106 O 0.6606(3) 0.7117(2) 0.40553(16) 0.0650(18) Uani 1 1 d . . . . .
O91 O 0.9463(4) 0.4873(2) 0.69370(18) 0.073(2) Uani 1 1 d . . . . .
O88 O 0.9503(5) 0.6075(3) 0.5027(2) 0.097(3) Uani 1 1 d . . . . .
O93 O 0.7611(4) 0.5294(2) 0.70244(17) 0.084(3) Uani 1 1 d . . . . .
O90 O 0.9822(6) 0.4151(3) 0.5607(2) 0.108(4) Uani 1 1 d . . . . .
O95 O 0.3096(5) 0.7200(4) 0.6384(3) 0.117(4) Uani 1 1 d . . . . .
O100 O 0.6699(5) 0.5948(2) 0.5275(3) 0.119(5) Uani 1 1 d . . . . .
O97 O 0.8437(6) 0.6817(4) 0.6568(4) 0.155(7) Uani 1 1 d . . . . .
O84 O 0.5310(5) 0.6989(4) 0.7862(5) 0.176(8) Uani 1 1 d . . . . .
O99 O 0.5827(6) 0.7455(6) 0.6338(3) 0.167(7) Uani 1 1 d . . . . .
O94 O 0.7098(5) 0.4481(3) 0.6729(2) 0.107(4) Uani 1 1 d . . . . .
O101 O 0.6944(6) 0.6650(4) 0.6007(2) 0.118(4) Uani 1 1 d . . . . .
O96 O 0.5445(5) 0.8913(3) 0.8043(2) 0.100(3) Uani 1 1 d . . . . .
O103 O 0.9421(6) 0.4536(4) 0.4979(2) 0.114(4) Uani 1 1 d . . . . .
O102 O 0.6067(5) 0.7273(3) 0.8591(2) 0.096(3) Uani 1 1 d . . . . .
O105 O 0.6508(6) 0.4990(3) 0.8758(2) 0.123(5) Uani 1 1 d . . . . .
O92 O 0.4882(5) 0.6009(4) 0.7999(4) 0.145(6) Uani 1 1 d . . . . .
Li1 Li 0.6240(7) 0.5023(5) 0.5428(4) 0.060(4) Uani 1 1 d . . . . .
Li4 Li 0.6265(9) 0.7073(6) 0.7077(3) 0.072(6) Uani 1 1 d . . . . .
O107 O 0.750000 0.750000 0.44834(19) 0.053(2) Uani 1 2 d S T P . .
Li6 Li 0.8321(9) 0.4865(5) 0.7379(4) 0.063(4) Uani 1 1 d . . . . .
Li8 Li 0.5265(9) 0.5655(5) 0.5188(5) 0.068(5) Uani 1 1 d . . . . .
Li10 Li 0.5486(8) 0.4600(5) 0.6932(4) 0.058(4) Uani 1 1 d . . . . .
Li12 Li 0.7993(8) 0.7114(6) 0.6026(4) 0.068(5) Uani 1 1 d . . . . .
Li14 Li 0.5114(7) 0.5334(5) 0.7449(4) 0.059(4) Uani 1 1 d . . . . .
O108 O 0.7371(8) 0.6325(3) 0.6734(3) 0.154(6) Uani 1 1 d . . . . .
Li16 Li 0.9074(10) 0.6058(5) 0.4227(4) 0.065(5) Uani 1 1 d . . . . .
Li18 Li 0.5025(9) 0.7618(8) 0.8965(4) 0.077(6) Uani 1 1 d . . . . .
Li20 Li 0.4569(9) 0.3654(8) 0.6147(4) 0.077(6) Uani 1 1 d . . . . .
Li22 Li 0.5095(16) 0.6188(6) 0.7005(10) 0.153(18) Uani 1 1 d . . . . .
Li24 Li 0.8334(8) 0.3778(6) 0.5505(4) 0.063(4) Uani 1 1 d . U . . .
Li3 Li 0.2545(9) 0.9024(7) 0.7411(7) 0.093(8) Uani 1 1 d . . . . .
Li13 Li 1.1213(9) 0.4956(8) 0.5664(4) 0.084(7) Uani 1 1 d . . . . .
Li7 Li 0.6980(12) 0.7208(6) 0.6517(4) 0.085(7) Uani 1 1 d . . . . .
Li15 Li 0.4271(9) 0.6601(6) 0.6274(4) 0.065(4) Uani 1 1 d . . . . .
Li2 Li 0.7318(8) 0.5761(4) 0.9107(3) 0.055(4) Uani 1 1 d . . . . .
Li17 Li 0.9309(9) 0.3549(5) 0.5161(5) 0.072(5) Uani 1 1 d . . . . .
Li9 Li 0.8439(12) 0.4126(7) 0.6948(4) 0.085(7) Uani 1 1 d . . . . .
Li19 Li 0.6933(9) 0.4213(6) 0.5899(6) 0.079(6) Uani 1 1 d . . . . .
Li5 Li 0.7188(5) 0.6513(3) 0.4500(2) 0.030(2) Uani 1 1 d . . . . .
Li21 Li 0.5880(14) 0.6545(8) 0.6459(5) 0.105(9) Uani 1 1 d . . . . .
Li11 Li 1.1717(11) 0.5656(9) 0.5341(5) 0.098(8) Uani 1 1 d . . . . .
Li23 Li 0.3381(11) 0.6580(9) 0.7062(7) 0.105(8) Uani 1 1 d . U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Nb1 Nb22 3.3425(11) . ?
Nb1 Nb7 3.3449(10) . ?
Nb1 O64 2.053(6) . ?
Nb1 O63 1.940(7) . ?
Nb1 O73 1.920(6) . ?
Nb1 O71 2.070(6) . ?
Nb1 O62 1.814(6) . ?
Nb1 O70 2.335(6) . ?
Nb4 Nb6 3.3095(10) . ?
Nb4 Nb8 3.3238(11) . ?
Nb4 Nb20 3.3564(10) . ?
Nb4 O54 2.407(6) . ?
Nb4 O53 2.007(7) . ?
Nb4 O50 1.996(6) . ?
Nb4 O47 1.995(6) . ?
Nb4 O80 1.981(6) . ?
Nb4 O52 1.797(7) . ?
Nb6 Nb20 3.3320(11) . ?
Nb6 O54 2.328(5) . ?
Nb6 O43 2.083(6) 2_665 ?
Nb6 O51 2.048(7) . ?
Nb6 O47 1.940(6) . ?
Nb6 O45 1.930(6) . ?
Nb6 O44 1.779(6) . ?
Nb8 Nb14 3.3167(11) . ?
Nb8 O54 2.341(6) . ?
Nb8 O51 2.057(6) . ?
Nb8 O53 1.940(6) . ?
Nb8 O58 1.922(6) . ?
Nb8 O41 2.061(6) 2_665 ?
Nb8 O59 1.818(7) . ?
Nb10 Nb14 3.3239(10) . ?
Nb10 Nb20 3.3475(13) . ?
Nb10 O54 2.383(6) . ?
Nb10 O43 2.079(6) 2_665 ?
Nb10 O41 2.059(7) 2_665 ?
Nb10 O56 1.918(6) . ?
Nb10 O49 1.928(7) . ?
Nb10 O55 1.783(7) . ?
Nb12 Nb2 3.3268(12) . ?
Nb12 Nb9 3.3363(12) . ?
Nb12 Fe4 3.1697(15) 2_665 ?
Nb12 O3 2.068(6) 2_665 ?
Nb12 O4 1.807(7) . ?
Nb12 O8 2.044(6) . ?
Nb12 O6 1.916(7) . ?
Nb12 O5 1.935(7) . ?
Nb12 O10 2.357(7) . ?
Nb14 Nb20 3.3402(11) . ?
Nb14 O54 2.412(5) . ?
Nb14 O75 1.971(7) . ?
Nb14 O58 2.025(7) . ?
Nb14 O80 1.991(6) . ?
Nb14 O56 2.007(7) . ?
Nb14 O57 1.752(7) . ?
Nb16 Nb22 3.3196(11) . ?
Nb16 Nb19 3.3337(12) . ?
Nb16 O64 2.043(6) . ?
Nb16 O68 2.070(7) . ?
Nb16 O66 1.916(7) . ?
Nb16 O70 2.308(6) . ?
Nb16 O1 1.787(7) . ?
Nb16 O67 1.938(7) . ?
Nb18 Nb2 3.3299(11) . ?
Nb18 Nb5 3.3236(12) . ?
Nb18 O8 2.072(7) . ?
Nb18 O14 2.079(7) . ?
Nb18 O10 2.344(6) . ?
Nb18 O11 1.916(8) . ?
Nb18 O9 1.927(7) . ?
Nb18 O20 1.806(7) . ?
Nb20 O54 2.394(6) . ?
Nb20 O50 1.974(6) . ?
Nb20 O75 1.960(7) . ?
Nb20 O45 2.005(6) . ?
Nb20 O49 2.034(7) . ?
Nb20 O48 1.777(8) . ?
Nb22 Nb7 3.3482(12) . ?
Nb22 Nb19 3.3476(12) . ?
Nb22 O63 2.037(6) . ?
Nb22 O66 2.018(7) . ?
Nb22 O72 1.952(7) . ?
Nb22 O70 2.385(7) . ?
Nb22 O69 1.952(7) . ?
Nb22 O65 1.792(8) . ?
Nb24 Nb9 3.3399(12) . ?
Nb24 Nb5 3.3335(13) . ?
Nb24 O3 2.074(7) 2_665 ?
Nb24 O14 2.050(6) . ?
Nb24 O13 1.916(8) . ?
Nb24 O16 1.946(7) . ?
Nb24 O10 2.375(7) . ?
Nb24 O15 1.781(7) . ?
Nb26 Nb21 3.3299(13) . ?
Nb26 O26 2.062(6) . ?
Nb26 O37 2.067(7) . ?
Nb26 O33 2.333(7) . ?
Nb26 O23 1.911(7) . ?
Nb26 O22 1.811(7) . ?
Nb26 O38 1.951(7) . ?
Nb26 Nb3 3.236(6) . ?
Nb13 Nb7 3.3318(12) . ?
Nb13 Nb19 3.3359(13) . ?
Nb13 O71 2.073(6) . ?
Nb13 O68 2.091(7) . ?
Nb13 O34 1.942(7) . ?
Nb13 O77 1.910(7) . ?
Nb13 O70 2.393(7) . ?
Nb13 O76 1.769(8) . ?
Nb7 Nb19 3.3450(12) . ?
Nb7 O73 2.003(6) . ?
Nb7 O34 2.004(7) . ?
Nb7 O72 1.986(8) . ?
Nb7 O70 2.418(6) . ?
Nb7 O79 1.950(7) . ?
Nb7 O74 1.780(7) . ?
Nb15 Nb11 3.244(2) . ?
Nb15 Nb23 3.355(2) . ?
Nb15 O37 2.057(7) . ?
Nb15 O60 2.066(6) 2_665 ?
Nb15 O40 1.799(8) . ?
Nb15 O33 2.313(7) . ?
Nb15 O39 1.919(8) . ?
Nb15 O31 1.922(8) . ?
Nb15 Nb25 3.245(5) . ?
Nb2 Nb9 3.3469(12) . ?
Nb2 Nb5 3.3537(14) . ?
Nb2 O6 2.040(7) . ?
Nb2 O10 2.395(7) . ?
Nb2 O9 2.026(7) . ?
Nb2 O46 1.972(8) . ?
Nb2 O19 1.964(7) . ?
Nb2 O7 1.757(8) . ?
Nb17 Nb21 3.3439(15) . ?
Nb17 Nb23 3.2986(17) . ?
Nb17 O26 2.073(6) . ?
Nb17 O60 2.051(7) 2_665 ?
Nb17 O33 2.359(7) . ?
Nb17 O25 1.933(9) . ?
Nb17 O27 1.762(9) . ?
Nb17 O29 1.914(7) . ?
Nb9 Nb5 3.3377(12) . ?
Nb9 O5 2.003(8) . ?
Nb9 O16 2.028(7) . ?
Nb9 O10 2.392(6) . ?
Nb9 O17 1.957(8) . ?
Nb9 O19 1.972(8) . ?
Nb9 O18 1.779(7) . ?
Nb19 O77 2.016(7) . ?
Nb19 O70 2.420(6) . ?
Nb19 O67 2.019(7) . ?
Nb19 O69 1.975(8) . ?
Nb19 O79 1.985(7) . ?
Nb19 O78 1.771(7) . ?
Nb5 O13 2.033(8) . ?
Nb5 O10 2.395(7) . ?
Nb5 O11 2.016(8) . ?
Nb5 O46 1.962(8) . ?
Nb5 O17 1.976(7) . ?
Nb5 O12 1.755(8) . ?
Nb21 Nb11 3.331(2) . ?
Nb21 O33 2.434(7) . ?
Nb21 O23 2.014(8) . ?
Nb21 O25 2.001(9) . ?
Nb21 O35 1.980(9) . ?
Nb21 O28 1.965(9) . ?
Nb21 O24 1.793(10) . ?
Nb21 Nb25 3.124(6) . ?
Nb11 Nb23 3.334(2) . ?
Nb11 O33 2.342(7) . ?
Nb11 O39 1.962(8) . ?
Nb11 O38 2.103(9) . ?
Nb11 O35 1.966(9) . ?
Nb11 O32 1.883(11) . ?
Nb11 O36 1.830(10) . ?
Nb23 O33 2.470(7) . ?
Nb23 O31 2.018(9) . ?
Nb23 O29 1.941(10) . ?
Nb23 O32 2.037(11) . ?
Nb23 O28 2.013(10) . ?
Nb23 O30 1.736(7) . ?
Fe1 O26 2.081(7) 2_665 ?
Fe1 O37 2.144(6) 2_665 ?
Fe1 O60 2.103(7) . ?
Fe1 O59 1.951(7) . ?
Fe1 O62 1.962(6) . ?
Fe1 O61 1.905(7) . ?
Fe4 O3 2.075(7) . ?
Fe4 O4 1.959(7) . ?
Fe4 O8 2.137(6) 2_665 ?
Fe4 O14 2.120(7) 2_665 ?
Fe4 O1 1.967(7) . ?
Fe4 O2 1.926(8) . ?
Fe2 O43 2.072(7) . ?
Fe2 O51 2.119(6) 2_665 ?
Fe2 O41 2.089(6) . ?
Fe2 O44 1.974(7) . ?
Fe2 O40 1.945(8) . ?
Fe2 O42 1.892(9) . ?
Fe3 O64 2.180(7) 2_665 ?
Fe3 O71 2.090(6) 2_665 ?
Fe3 O68 2.063(7) 2_665 ?
Fe3 O22 1.953(7) . ?
Fe3 O20 1.952(7) . ?
Fe3 O21 1.915(8) . ?
O5 Li5 2.609(12) . ?
O33 Nb25 2.186(8) . ?
O69 Li1 2.677(16) . ?
O48 Li16 2.648(17) 8_756 ?
O55 Li20 2.663(19) 4_566 ?
O39 Nb3 2.164(10) . ?
O38 Nb3 1.705(10) . ?
O31 Nb25 2.144(10) . ?
O29 Nb25 2.364(11) . ?
O35 Nb3 1.953(10) . ?
O32 Nb3 2.444(13) . ?
O32 Nb25 1.517(12) . ?
O2 Li5 2.547(16) . ?
O28 Nb25 1.859(10) . ?
O36 Nb3 1.617(10) . ?
O30 Nb25 2.100(9) . ?
Nb3 Nb25 3.323(6) . ?
O93 Li6 2.62(2) . ?
O105 Li13 2.603(18) 4_466 ?
Li1 Li8 3.18(3) . ?
Li4 Li7 2.95(3) . ?
Li4 Li21 3.30(3) . ?
Li6 Li3 3.48(3) 3_646 ?
Li6 Li9 3.05(2) . ?
Li10 Li14 3.38(3) . ?
Li12 Li12 3.35(4) 2_665 ?
Li12 Li7 3.14(2) . ?
Li12 Li7 3.06(3) 2_665 ?
Li14 Li22 3.37(3) . ?
Li16 Li13 3.38(3) 5_766 ?
Li16 Li2 3.33(3) 8_755 ?
Li18 Li20 3.52(4) 3_656 ?
Li22 Li21 3.18(5) . ?
Li24 Li17 2.76(3) . ?
Li3 Li23 3.24(3) 2_565 ?
Li13 Li11 2.90(4) . ?
Li7 Li7 3.02(5) 2_665 ?
Li7 Li21 3.29(3) . ?
Li2 Li5 3.177(17) 8_756 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Nb22 Nb1 Nb7 60.09(2) . . ?
O64 Nb1 Nb22 84.86(19) . . ?
O64 Nb1 Nb7 123.10(18) . . ?
O64 Nb1 O71 79.0(3) . . ?
O64 Nb1 O70 76.9(2) . . ?
O63 Nb1 Nb22 33.73(18) . . ?
O63 Nb1 Nb7 83.85(18) . . ?
O63 Nb1 O64 89.7(3) . . ?
O63 Nb1 O71 155.5(3) . . ?
O63 Nb1 O70 79.1(2) . . ?
O73 Nb1 Nb22 82.8(2) . . ?
O73 Nb1 Nb7 32.27(18) . . ?
O73 Nb1 O64 154.5(3) . . ?
O73 Nb1 O63 92.4(3) . . ?
O73 Nb1 O71 89.0(3) . . ?
O73 Nb1 O70 78.5(2) . . ?
O71 Nb1 Nb22 122.61(18) . . ?
O71 Nb1 Nb7 84.30(17) . . ?
O71 Nb1 O70 77.2(2) . . ?
O62 Nb1 Nb22 136.8(2) . . ?
O62 Nb1 Nb7 133.55(19) . . ?
O62 Nb1 O64 103.0(3) . . ?
O62 Nb1 O63 103.2(3) . . ?
O62 Nb1 O73 101.3(3) . . ?
O62 Nb1 O71 100.6(3) . . ?
O62 Nb1 O70 177.7(3) . . ?
O70 Nb1 Nb22 45.52(16) . . ?
O70 Nb1 Nb7 46.30(15) . . ?
Nb6 Nb4 Nb8 61.74(2) . . ?
Nb6 Nb4 Nb20 59.98(2) . . ?
Nb8 Nb4 Nb20 90.20(3) . . ?
O54 Nb4 Nb6 44.69(13) . . ?
O54 Nb4 Nb8 44.76(15) . . ?
O54 Nb4 Nb20 45.49(15) . . ?
O53 Nb4 Nb6 81.26(16) . . ?
O53 Nb4 Nb8 32.03(18) . . ?
O53 Nb4 Nb20 122.19(18) . . ?
O53 Nb4 O54 76.7(2) . . ?
O50 Nb4 Nb6 80.05(18) . . ?
O50 Nb4 Nb8 122.3(2) . . ?
O50 Nb4 Nb20 32.1(2) . . ?
O50 Nb4 O54 77.5(2) . . ?
O50 Nb4 O53 154.2(3) . . ?
O47 Nb4 Nb6 32.25(18) . . ?
O47 Nb4 Nb8 81.99(19) . . ?
O47 Nb4 Nb20 81.97(18) . . ?
O47 Nb4 O54 76.9(2) . . ?
O47 Nb4 O53 86.2(3) . . ?
O47 Nb4 O50 87.4(3) . . ?
O80 Nb4 Nb6 122.06(18) . . ?
O80 Nb4 Nb8 79.04(19) . . ?
O80 Nb4 Nb20 80.85(17) . . ?
O80 Nb4 O54 77.4(2) . . ?
O80 Nb4 O53 86.9(3) . . ?
O80 Nb4 O50 88.2(3) . . ?
O80 Nb4 O47 154.3(3) . . ?
O52 Nb4 Nb6 134.6(2) . . ?
O52 Nb4 Nb8 135.5(2) . . ?
O52 Nb4 Nb20 134.3(2) . . ?
O52 Nb4 O54 179.3(3) . . ?
O52 Nb4 O53 103.5(3) . . ?
O52 Nb4 O50 102.2(3) . . ?
O52 Nb4 O47 102.4(3) . . ?
O52 Nb4 O80 103.3(3) . . ?
Nb4 Nb6 Nb20 60.71(2) . . ?
O54 Nb6 Nb4 46.64(16) . . ?
O54 Nb6 Nb20 45.93(16) . . ?
O43 Nb6 Nb4 123.22(16) 2_665 . ?
O43 Nb6 Nb20 84.55(18) 2_665 . ?
O43 Nb6 O54 76.7(2) 2_665 . ?
O51 Nb6 Nb4 84.81(17) . . ?
O51 Nb6 Nb20 122.80(17) . . ?
O51 Nb6 O54 77.0(2) . . ?
O51 Nb6 O43 78.2(3) . 2_665 ?
O47 Nb6 Nb4 33.26(18) . . ?
O47 Nb6 Nb20 83.37(19) . . ?
O47 Nb6 O54 79.9(2) . . ?
O47 Nb6 O43 155.8(3) . 2_665 ?
O47 Nb6 O51 90.9(3) . . ?
O45 Nb6 Nb4 83.70(19) . . ?
O45 Nb6 Nb20 32.84(19) . . ?
O45 Nb6 O54 78.6(2) . . ?
O45 Nb6 O43 89.3(3) . 2_665 ?
O45 Nb6 O51 154.6(3) . . ?
O45 Nb6 O47 91.8(3) . . ?
O44 Nb6 Nb4 136.8(2) . . ?
O44 Nb6 Nb20 133.1(2) . . ?
O44 Nb6 O54 176.4(3) . . ?
O44 Nb6 O43 100.0(3) . 2_665 ?
O44 Nb6 O51 103.7(3) . . ?
O44 Nb6 O47 103.6(3) . . ?
O44 Nb6 O45 100.2(3) . . ?
Nb14 Nb8 Nb4 61.14(2) . . ?
O54 Nb8 Nb4 46.39(16) . . ?
O54 Nb8 Nb14 46.62(13) . . ?
O51 Nb8 Nb4 84.31(19) . . ?
O51 Nb8 Nb14 123.03(18) . . ?
O51 Nb8 O54 76.5(2) . . ?
O51 Nb8 O41 78.4(2) . 2_665 ?
O53 Nb8 Nb4 33.28(19) . . ?
O53 Nb8 Nb14 84.12(19) . . ?
O53 Nb8 O54 79.6(2) . . ?
O53 Nb8 O51 89.8(3) . . ?
O53 Nb8 O41 155.5(3) . 2_665 ?
O58 Nb8 Nb4 85.5(2) . . ?
O58 Nb8 Nb14 33.80(19) . . ?
O58 Nb8 O54 80.2(2) . . ?
O58 Nb8 O51 155.4(3) . . ?
O58 Nb8 O53 93.9(3) . . ?
O58 Nb8 O41 88.6(3) . 2_665 ?
O41 Nb8 Nb4 123.08(19) 2_665 . ?
O41 Nb8 Nb14 84.53(18) 2_665 . ?
O41 Nb8 O54 76.8(3) 2_665 . ?
O59 Nb8 Nb4 135.2(2) . . ?
O59 Nb8 Nb14 134.3(2) . . ?
O59 Nb8 O54 178.2(3) . . ?
O59 Nb8 O51 102.4(3) . . ?
O59 Nb8 O53 101.9(3) . . ?
O59 Nb8 O58 100.6(3) . . ?
O59 Nb8 O41 101.6(3) . 2_665 ?
Nb14 Nb10 Nb20 60.09(2) . . ?
O54 Nb10 Nb14 46.47(13) . . ?
O54 Nb10 Nb20 45.65(15) . . ?
O43 Nb10 Nb14 121.90(17) 2_665 . ?
O43 Nb10 Nb20 84.2(2) 2_665 . ?
O43 Nb10 O54 75.6(2) 2_665 . ?
O41 Nb10 Nb14 84.37(17) 2_665 . ?
O41 Nb10 Nb20 121.45(18) 2_665 . ?
O41 Nb10 O54 75.9(2) 2_665 . ?
O41 Nb10 O43 77.2(3) 2_665 2_665 ?
O56 Nb10 Nb14 32.9(2) . . ?
O56 Nb10 Nb20 83.4(2) . . ?
O56 Nb10 O54 79.3(2) . . ?
O56 Nb10 O43 153.8(3) . 2_665 ?
O56 Nb10 O41 89.8(3) . 2_665 ?
O56 Nb10 O49 93.0(3) . . ?
O49 Nb10 Nb14 83.81(18) . . ?
O49 Nb10 Nb20 33.31(18) . . ?
O49 Nb10 O54 78.8(2) . . ?
O49 Nb10 O43 89.2(3) . 2_665 ?
O49 Nb10 O41 153.5(3) . 2_665 ?
O55 Nb10 Nb14 136.7(2) . . ?
O55 Nb10 Nb20 137.6(3) . . ?
O55 Nb10 O54 175.4(3) . . ?
O55 Nb10 O43 100.9(3) . 2_665 ?
O55 Nb10 O41 100.6(3) . 2_665 ?
O55 Nb10 O56 103.8(3) . . ?
O55 Nb10 O49 104.3(3) . . ?
Nb2 Nb12 Nb9 60.30(3) . . ?
Fe4 Nb12 Nb2 117.11(4) 2_665 . ?
Fe4 Nb12 Nb9 116.42(4) 2_665 . ?
O3 Nb12 Nb2 122.66(19) 2_665 . ?
O3 Nb12 Nb9 84.49(19) 2_665 . ?
O3 Nb12 Fe4 40.18(18) 2_665 2_665 ?
O3 Nb12 O10 76.7(3) 2_665 . ?
O4 Nb12 Nb2 138.0(2) . . ?
O4 Nb12 Nb9 132.5(2) . . ?
O4 Nb12 Fe4 93.3(2) . 2_665 ?
O4 Nb12 O3 99.3(3) . 2_665 ?
O4 Nb12 O8 104.1(3) . . ?
O4 Nb12 O6 104.2(3) . . ?
O4 Nb12 O5 99.8(3) . . ?
O4 Nb12 O10 175.6(3) . . ?
O8 Nb12 Nb2 84.29(18) . . ?
O8 Nb12 Nb9 122.89(19) . . ?
O8 Nb12 Fe4 41.81(17) . 2_665 ?
O8 Nb12 O3 79.0(2) . 2_665 ?
O8 Nb12 O10 77.2(2) . . ?
O6 Nb12 Nb2 33.9(2) . . ?
O6 Nb12 Nb9 83.4(2) . . ?
O6 Nb12 Fe4 132.0(2) . 2_665 ?
O6 Nb12 O3 156.0(3) . 2_665 ?
O6 Nb12 O8 90.3(3) . . ?
O6 Nb12 O5 91.8(3) . . ?
O6 Nb12 O10 79.9(3) . . ?
O5 Nb12 Nb2 83.4(2) . . ?
O5 Nb12 Nb9 32.7(2) . . ?
O5 Nb12 Fe4 129.2(2) . 2_665 ?
O5 Nb12 O3 89.2(3) . 2_665 ?
O5 Nb12 O8 154.7(3) . . ?
O5 Nb12 O10 78.4(3) . . ?
O10 Nb12 Nb2 46.04(17) . . ?
O10 Nb12 Nb9 45.80(15) . . ?
O10 Nb12 Fe4 84.95(16) . 2_665 ?
Nb8 Nb14 Nb10 62.28(2) . . ?
Nb8 Nb14 Nb20 90.60(3) . . ?
Nb10 Nb14 Nb20 60.31(2) . . ?
O54 Nb14 Nb8 44.87(15) . . ?
O54 Nb14 Nb10 45.75(15) . . ?
O54 Nb14 Nb20 45.76(15) . . ?
O75 Nb14 Nb8 122.31(19) . . ?
O75 Nb14 Nb10 79.55(19) . . ?
O75 Nb14 Nb20 31.71(18) . . ?
O75 Nb14 O54 77.4(2) . . ?
O75 Nb14 O58 153.8(3) . . ?
O75 Nb14 O80 88.8(3) . . ?
O75 Nb14 O56 87.8(3) . . ?
O58 Nb14 Nb8 31.87(18) . . ?
O58 Nb14 Nb10 80.20(16) . . ?
O58 Nb14 Nb20 122.30(18) . . ?
O58 Nb14 O54 76.6(2) . . ?
O80 Nb14 Nb8 79.10(19) . . ?
O80 Nb14 Nb10 122.83(18) . . ?
O80 Nb14 Nb20 81.15(18) . . ?
O80 Nb14 O54 77.1(2) . . ?
O80 Nb14 O58 88.4(3) . . ?
O80 Nb14 O56 153.9(3) . . ?
O56 Nb14 Nb8 81.0(2) . . ?
O56 Nb14 Nb10 31.31(18) . . ?
O56 Nb14 Nb20 82.4(2) . . ?
O56 Nb14 O54 77.0(2) . . ?
O56 Nb14 O58 83.5(3) . . ?
O57 Nb14 Nb8 135.3(3) . . ?
O57 Nb14 Nb10 135.1(3) . . ?
O57 Nb14 Nb20 134.0(3) . . ?
O57 Nb14 O54 179.1(3) . . ?
O57 Nb14 O75 102.3(3) . . ?
O57 Nb14 O58 103.7(3) . . ?
O57 Nb14 O80 102.1(3) . . ?
O57 Nb14 O56 103.9(3) . . ?
Nb22 Nb16 Nb19 60.42(3) . . ?
O64 Nb16 Nb22 85.62(18) . . ?
O64 Nb16 Nb19 124.17(17) . . ?
O64 Nb16 O68 78.8(3) . . ?
O64 Nb16 O70 77.8(2) . . ?
O68 Nb16 Nb22 124.07(18) . . ?
O68 Nb16 Nb19 85.5(2) . . ?
O68 Nb16 O70 78.2(2) . . ?
O66 Nb16 Nb22 33.4(2) . . ?
O66 Nb16 Nb19 83.2(2) . . ?
O66 Nb16 O64 91.0(3) . . ?
O66 Nb16 O68 156.8(3) . . ?
O66 Nb16 O70 79.3(3) . . ?
O66 Nb16 O67 91.7(3) . . ?
O70 Nb16 Nb22 45.92(17) . . ?
O70 Nb16 Nb19 46.55(15) . . ?
O1 Nb16 Nb22 136.1(2) . . ?
O1 Nb16 Nb19 133.9(3) . . ?
O1 Nb16 O64 101.6(3) . . ?
O1 Nb16 O68 99.8(3) . . ?
O1 Nb16 O66 102.7(3) . . ?
O1 Nb16 O70 178.0(3) . . ?
O1 Nb16 O67 100.6(3) . . ?
O67 Nb16 Nb22 83.9(2) . . ?
O67 Nb16 Nb19 33.4(2) . . ?
O67 Nb16 O64 156.5(3) . . ?
O67 Nb16 O68 89.8(3) . . ?
O67 Nb16 O70 79.8(3) . . ?
Nb5 Nb18 Nb2 60.54(3) . . ?
O8 Nb18 Nb2 83.80(17) . . ?
O8 Nb18 Nb5 122.98(17) . . ?
O8 Nb18 O14 79.5(2) . . ?
O8 Nb18 O10 77.0(2) . . ?
O14 Nb18 Nb2 123.09(17) . . ?
O14 Nb18 Nb5 84.78(19) . . ?
O14 Nb18 O10 77.2(2) . . ?
O10 Nb18 Nb2 46.00(17) . . ?
O10 Nb18 Nb5 46.09(17) . . ?
O11 Nb18 Nb2 83.5(2) . . ?
O11 Nb18 Nb5 33.2(2) . . ?
O11 Nb18 O8 155.6(3) . . ?
O11 Nb18 O14 90.1(3) . . ?
O11 Nb18 O10 79.2(3) . . ?
O11 Nb18 O9 91.7(3) . . ?
O9 Nb18 Nb2 33.5(2) . . ?
O9 Nb18 Nb5 83.6(2) . . ?
O9 Nb18 O8 89.2(3) . . ?
O9 Nb18 O14 155.9(3) . . ?
O9 Nb18 O10 79.5(3) . . ?
O20 Nb18 Nb2 137.0(3) . . ?
O20 Nb18 Nb5 134.1(3) . . ?
O20 Nb18 O8 102.6(3) . . ?
O20 Nb18 O14 99.8(3) . . ?
O20 Nb18 O10 177.0(3) . . ?
O20 Nb18 O11 100.9(3) . . ?
O20 Nb18 O9 103.5(3) . . ?
Nb6 Nb20 Nb4 59.31(2) . . ?
Nb6 Nb20 Nb10 62.37(2) . . ?
Nb6 Nb20 Nb14 90.49(3) . . ?
Nb10 Nb20 Nb4 91.13(3) . . ?
Nb14 Nb20 Nb4 60.57(2) . . ?
Nb14 Nb20 Nb10 59.60(2) . . ?
O54 Nb20 Nb4 45.80(15) . . ?
O54 Nb20 Nb6 44.33(13) . . ?
O54 Nb20 Nb10 45.37(15) . . ?
O54 Nb20 Nb14 46.18(13) . . ?
O50 Nb20 Nb4 32.5(2) . . ?
O50 Nb20 Nb6 79.74(19) . . ?
O50 Nb20 Nb10 123.6(2) . . ?
O50 Nb20 Nb14 82.2(2) . . ?
O50 Nb20 O54 78.3(3) . . ?
O50 Nb20 O45 87.6(3) . . ?
O50 Nb20 O49 154.8(3) . . ?
O75 Nb20 Nb4 82.09(18) . . ?
O75 Nb20 Nb6 122.4(2) . . ?
O75 Nb20 Nb10 79.1(2) . . ?
O75 Nb20 Nb14 31.9(2) . . ?
O75 Nb20 O54 78.1(2) . . ?
O75 Nb20 O50 89.4(3) . . ?
O75 Nb20 O45 153.6(3) . . ?
O75 Nb20 O49 87.4(3) . . ?
O45 Nb20 Nb4 81.41(17) . . ?
O45 Nb20 Nb6 31.47(18) . . ?
O45 Nb20 Nb10 80.9(2) . . ?
O45 Nb20 Nb14 121.85(18) . . ?
O45 Nb20 O54 75.7(2) . . ?
O45 Nb20 O49 84.3(3) . . ?
O49 Nb20 Nb4 122.38(19) . . ?
O49 Nb20 Nb6 80.90(18) . . ?
O49 Nb20 Nb10 31.38(19) . . ?
O49 Nb20 Nb14 81.92(18) . . ?
O49 Nb20 O54 76.6(2) . . ?
O48 Nb20 Nb4 135.2(3) . . ?
O48 Nb20 Nb6 133.8(3) . . ?
O48 Nb20 Nb10 133.6(3) . . ?
O48 Nb20 Nb14 135.7(3) . . ?
O48 Nb20 O54 177.9(3) . . ?
O48 Nb20 O50 102.8(3) . . ?
O48 Nb20 O75 103.8(3) . . ?
O48 Nb20 O45 102.4(3) . . ?
O48 Nb20 O49 102.3(3) . . ?
Nb1 Nb22 Nb7 59.99(2) . . ?
Nb1 Nb22 Nb19 90.55(3) . . ?
Nb16 Nb22 Nb1 60.97(2) . . ?
Nb16 Nb22 Nb7 90.23(3) . . ?
Nb16 Nb22 Nb19 60.00(3) . . ?
Nb19 Nb22 Nb7 59.94(3) . . ?
O63 Nb22 Nb1 31.92(18) . . ?
O63 Nb22 Nb16 80.10(16) . . ?
O63 Nb22 Nb7 82.42(18) . . ?
O63 Nb22 Nb19 122.39(18) . . ?
O63 Nb22 O70 76.1(2) . . ?
O66 Nb22 Nb1 80.41(19) . . ?
O66 Nb22 Nb16 31.52(19) . . ?
O66 Nb22 Nb7 121.7(2) . . ?
O66 Nb22 Nb19 81.4(2) . . ?
O66 Nb22 O63 84.4(3) . . ?
O66 Nb22 O70 75.5(2) . . ?
O72 Nb22 Nb1 80.0(2) . . ?
O72 Nb22 Nb16 122.3(2) . . ?
O72 Nb22 Nb7 32.1(2) . . ?
O72 Nb22 Nb19 81.4(2) . . ?
O72 Nb22 O63 88.2(3) . . ?
O72 Nb22 O66 153.7(3) . . ?
O72 Nb22 O70 78.2(3) . . ?
O70 Nb22 Nb1 44.32(14) . . ?
O70 Nb22 Nb16 44.05(14) . . ?
O70 Nb22 Nb7 46.22(14) . . ?
O70 Nb22 Nb19 46.27(14) . . ?
O69 Nb22 Nb1 122.3(2) . . ?
O69 Nb22 Nb16 79.9(2) . . ?
O69 Nb22 Nb7 81.2(2) . . ?
O69 Nb22 Nb19 31.7(2) . . ?
O69 Nb22 O63 154.0(3) . . ?
O69 Nb22 O66 87.2(3) . . ?
O69 Nb22 O72 88.6(3) . . ?
O69 Nb22 O70 77.9(3) . . ?
O65 Nb22 Nb1 133.9(2) . . ?
O65 Nb22 Nb16 134.9(3) . . ?
O65 Nb22 Nb7 134.9(3) . . ?
O65 Nb22 Nb19 135.5(2) . . ?
O65 Nb22 O63 102.1(3) . . ?
O65 Nb22 O66 103.4(3) . . ?
O65 Nb22 O72 102.8(4) . . ?
O65 Nb22 O70 177.9(3) . . ?
O65 Nb22 O69 103.8(3) . . ?
Nb5 Nb24 Nb9 60.02(3) . . ?
O3 Nb24 Nb9 84.31(17) 2_665 . ?
O3 Nb24 Nb5 122.04(17) 2_665 . ?
O3 Nb24 O10 76.2(2) 2_665 . ?
O14 Nb24 Nb9 122.65(18) . . ?
O14 Nb24 Nb5 84.9(2) . . ?
O14 Nb24 O3 77.9(3) . 2_665 ?
O14 Nb24 O10 77.0(2) . . ?
O13 Nb24 Nb9 84.0(2) . . ?
O13 Nb24 Nb5 33.5(2) . . ?
O13 Nb24 O3 154.4(3) . 2_665 ?
O13 Nb24 O14 89.5(3) . . ?
O13 Nb24 O16 93.0(3) . . ?
O13 Nb24 O10 79.3(3) . . ?
O16 Nb24 Nb9 33.6(2) . . ?
O16 Nb24 Nb5 83.6(2) . . ?
O16 Nb24 O3 89.7(3) . 2_665 ?
O16 Nb24 O14 155.2(3) . . ?
O16 Nb24 O10 79.2(3) . . ?
O10 Nb24 Nb9 45.73(15) . . ?
O10 Nb24 Nb5 45.90(17) . . ?
O15 Nb24 Nb9 137.0(2) . . ?
O15 Nb24 Nb5 138.2(3) . . ?
O15 Nb24 O3 99.4(3) . 2_665 ?
O15 Nb24 O14 99.8(3) . . ?
O15 Nb24 O13 104.7(4) . . ?
O15 Nb24 O16 103.4(3) . . ?
O15 Nb24 O10 175.0(3) . . ?
O26 Nb26 Nb21 85.1(2) . . ?
O26 Nb26 O37 78.6(3) . . ?
O26 Nb26 O33 76.9(2) . . ?
O26 Nb26 Nb3 130.7(2) . . ?
O37 Nb26 Nb21 124.10(19) . . ?
O37 Nb26 O33 77.2(3) . . ?
O37 Nb26 Nb3 88.0(2) . . ?
O33 Nb26 Nb21 46.94(18) . . ?
O33 Nb26 Nb3 53.8(2) . . ?
O23 Nb26 Nb21 32.9(2) . . ?
O23 Nb26 O26 89.6(3) . . ?
O23 Nb26 O37 156.0(3) . . ?
O23 Nb26 O33 79.7(3) . . ?
O23 Nb26 O38 92.5(3) . . ?
O23 Nb26 Nb3 83.9(2) . . ?
O22 Nb26 Nb21 134.4(2) . . ?
O22 Nb26 O26 100.0(3) . . ?
O22 Nb26 O37 101.1(3) . . ?
O22 Nb26 O33 176.7(3) . . ?
O22 Nb26 O23 101.5(3) . . ?
O22 Nb26 O38 103.7(3) . . ?
O22 Nb26 Nb3 129.2(2) . . ?
O38 Nb26 Nb21 83.4(2) . . ?
O38 Nb26 O26 155.3(3) . . ?
O38 Nb26 O37 89.8(3) . . ?
O38 Nb26 O33 79.2(3) . . ?
O38 Nb26 Nb3 25.8(3) . . ?
Nb3 Nb26 Nb21 63.87(10) . . ?
Nb7 Nb13 Nb19 60.22(3) . . ?
O71 Nb13 Nb7 84.60(17) . . ?
O71 Nb13 Nb19 122.18(18) . . ?
O71 Nb13 O68 76.8(2) . . ?
O71 Nb13 O70 75.8(2) . . ?
O68 Nb13 Nb7 122.27(18) . . ?
O68 Nb13 Nb19 85.08(19) . . ?
O68 Nb13 O70 75.9(2) . . ?
O34 Nb13 Nb7 33.0(2) . . ?
O34 Nb13 Nb19 83.2(2) . . ?
O34 Nb13 O71 90.2(3) . . ?
O34 Nb13 O68 154.2(3) . . ?
O34 Nb13 O70 79.3(3) . . ?
O77 Nb13 Nb7 83.8(2) . . ?
O77 Nb13 Nb19 32.8(2) . . ?
O77 Nb13 O71 153.7(3) . . ?
O77 Nb13 O68 89.7(3) . . ?
O77 Nb13 O34 92.8(3) . . ?
O77 Nb13 O70 79.0(3) . . ?
O70 Nb13 Nb7 46.48(14) . . ?
O70 Nb13 Nb19 46.46(14) . . ?
O76 Nb13 Nb7 136.9(3) . . ?
O76 Nb13 Nb19 136.1(3) . . ?
O76 Nb13 O71 101.3(3) . . ?
O76 Nb13 O68 100.4(3) . . ?
O76 Nb13 O34 103.9(3) . . ?
O76 Nb13 O77 103.4(3) . . ?
O76 Nb13 O70 175.7(3) . . ?
Nb1 Nb7 Nb22 59.92(2) . . ?
Nb1 Nb7 Nb19 90.56(3) . . ?
Nb13 Nb7 Nb1 62.13(2) . . ?
Nb13 Nb7 Nb22 91.18(3) . . ?
Nb13 Nb7 Nb19 59.95(3) . . ?
Nb19 Nb7 Nb22 60.02(3) . . ?
O73 Nb7 Nb1 30.77(17) . . ?
O73 Nb7 Nb22 81.53(19) . . ?
O73 Nb7 Nb13 80.18(18) . . ?
O73 Nb7 Nb19 121.24(18) . . ?
O73 Nb7 O34 84.6(3) . . ?
O73 Nb7 O70 75.0(2) . . ?
O34 Nb7 Nb1 81.44(18) . . ?
O34 Nb7 Nb22 122.95(19) . . ?
O34 Nb7 Nb13 31.82(18) . . ?
O34 Nb7 Nb19 82.14(19) . . ?
O34 Nb7 O70 77.6(2) . . ?
O72 Nb7 Nb1 79.51(19) . . ?
O72 Nb7 Nb22 31.45(19) . . ?
O72 Nb7 Nb13 122.63(19) . . ?
O72 Nb7 Nb19 81.0(2) . . ?
O72 Nb7 O73 87.7(3) . . ?
O72 Nb7 O34 154.3(3) . . ?
O72 Nb7 O70 76.8(2) . . ?
O70 Nb7 Nb1 44.28(14) . . ?
O70 Nb7 Nb22 45.40(16) . . ?
O70 Nb7 Nb13 45.85(16) . . ?
O70 Nb7 Nb19 46.29(14) . . ?
O79 Nb7 Nb1 122.7(2) . . ?
O79 Nb7 Nb22 81.2(2) . . ?
O79 Nb7 Nb13 80.0(2) . . ?
O79 Nb7 Nb19 32.1(2) . . ?
O79 Nb7 O73 153.3(3) . . ?
O79 Nb7 O34 87.9(3) . . ?
O79 Nb7 O72 88.1(3) . . ?
O79 Nb7 O70 78.4(3) . . ?
O74 Nb7 Nb1 133.6(2) . . ?
O74 Nb7 Nb22 134.4(3) . . ?
O74 Nb7 Nb13 134.5(3) . . ?
O74 Nb7 Nb19 135.8(2) . . ?
O74 Nb7 O73 102.9(3) . . ?
O74 Nb7 O34 102.7(3) . . ?
O74 Nb7 O72 102.9(3) . . ?
O74 Nb7 O70 177.9(3) . . ?
O74 Nb7 O79 103.7(3) . . ?
Nb11 Nb15 Nb23 60.66(5) . . ?
O37 Nb15 Nb11 87.70(18) . . ?
O37 Nb15 Nb23 125.0(2) . . ?
O37 Nb15 O60 78.9(3) . 2_665 ?
O37 Nb15 O33 77.9(3) . . ?
O37 Nb15 Nb25 119.9(2) . . ?
O60 Nb15 Nb11 122.4(2) 2_665 . ?
O60 Nb15 Nb23 82.45(19) 2_665 . ?
O60 Nb15 O33 76.2(3) 2_665 . ?
O60 Nb15 Nb25 89.6(2) 2_665 . ?
O40 Nb15 Nb11 135.7(2) . . ?
O40 Nb15 Nb23 132.8(3) . . ?
O40 Nb15 O37 101.7(3) . . ?
O40 Nb15 O60 101.9(3) . 2_665 ?
O40 Nb15 O33 178.1(3) . . ?
O40 Nb15 O39 102.3(3) . . ?
O40 Nb15 O31 100.3(4) . . ?
O40 Nb15 Nb25 138.3(3) . . ?
O33 Nb15 Nb11 46.19(17) . . ?
O33 Nb15 Nb23 47.39(18) . . ?
O33 Nb15 Nb25 42.3(2) . . ?
O39 Nb15 Nb11 33.7(2) . . ?
O39 Nb15 Nb23 85.3(2) . . ?
O39 Nb15 O37 90.7(3) . . ?
O39 Nb15 O60 155.1(3) . 2_665 ?
O39 Nb15 O33 79.6(3) . . ?
O39 Nb15 O31 93.3(4) . . ?
O39 Nb15 Nb25 76.0(3) . . ?
O31 Nb15 Nb11 82.8(3) . . ?
O31 Nb15 Nb23 32.5(3) . . ?
O31 Nb15 O37 156.2(3) . . ?
O31 Nb15 O60 87.9(3) . 2_665 ?
O31 Nb15 O33 79.8(3) . . ?
O31 Nb15 Nb25 39.5(3) . . ?
Nb12 Nb2 Nb18 61.73(2) . . ?
Nb12 Nb2 Nb9 59.99(3) . . ?
Nb12 Nb2 Nb5 90.64(3) . . ?
Nb18 Nb2 Nb9 90.30(3) . . ?
Nb18 Nb2 Nb5 59.64(3) . . ?
Nb9 Nb2 Nb5 59.75(3) . . ?
O6 Nb2 Nb12 31.62(18) . . ?
O6 Nb2 Nb18 81.59(19) . . ?
O6 Nb2 Nb9 81.46(19) . . ?
O6 Nb2 Nb5 122.25(19) . . ?
O6 Nb2 O10 76.7(3) . . ?
O10 Nb2 Nb12 45.11(17) . . ?
O10 Nb2 Nb18 44.73(15) . . ?
O10 Nb2 Nb9 45.60(15) . . ?
O10 Nb2 Nb5 45.55(17) . . ?
O9 Nb2 Nb12 81.1(2) . . ?
O9 Nb2 Nb18 31.7(2) . . ?
O9 Nb2 Nb9 122.0(2) . . ?
O9 Nb2 Nb5 81.5(2) . . ?
O9 Nb2 O6 86.1(3) . . ?
O9 Nb2 O10 76.4(2) . . ?
O46 Nb2 Nb12 122.0(2) . . ?
O46 Nb2 Nb18 78.6(2) . . ?
O46 Nb2 Nb9 81.3(2) . . ?
O46 Nb2 Nb5 31.4(2) . . ?
O46 Nb2 O6 153.6(3) . . ?
O46 Nb2 O10 76.9(3) . . ?
O46 Nb2 O9 86.2(3) . . ?
O19 Nb2 Nb12 79.7(2) . . ?
O19 Nb2 Nb18 122.1(2) . . ?
O19 Nb2 Nb9 31.8(2) . . ?
O19 Nb2 Nb5 81.1(2) . . ?
O19 Nb2 O6 86.8(3) . . ?
O19 Nb2 O10 77.4(3) . . ?
O19 Nb2 O9 153.8(3) . . ?
O19 Nb2 O46 89.0(3) . . ?
O7 Nb2 Nb12 134.1(3) . . ?
O7 Nb2 Nb18 134.9(3) . . ?
O7 Nb2 Nb9 134.8(3) . . ?
O7 Nb2 Nb5 135.3(3) . . ?
O7 Nb2 O6 102.5(4) . . ?
O7 Nb2 O10 179.1(4) . . ?
O7 Nb2 O9 103.2(3) . . ?
O7 Nb2 O46 103.9(4) . . ?
O7 Nb2 O19 103.0(4) . . ?
Nb23 Nb17 Nb21 62.18(5) . . ?
O26 Nb17 Nb21 84.58(19) . . ?
O26 Nb17 Nb23 124.31(17) . . ?
O26 Nb17 O33 76.1(2) . . ?
O60 Nb17 Nb21 122.03(19) 2_665 . ?
O60 Nb17 Nb23 84.14(18) 2_665 . ?
O60 Nb17 O26 77.4(3) 2_665 . ?
O60 Nb17 O33 75.5(3) 2_665 . ?
O33 Nb17 Nb21 46.68(18) . . ?
O33 Nb17 Nb23 48.33(18) . . ?
O25 Nb17 Nb21 32.4(2) . . ?
O25 Nb17 Nb23 84.3(2) . . ?
O25 Nb17 O26 89.6(3) . . ?
O25 Nb17 O60 153.4(3) . 2_665 ?
O25 Nb17 O33 79.0(3) . . ?
O27 Nb17 Nb21 137.9(3) . . ?
O27 Nb17 Nb23 134.3(3) . . ?
O27 Nb17 O26 100.7(3) . . ?
O27 Nb17 O60 99.7(4) . 2_665 ?
O27 Nb17 O33 174.6(3) . . ?
O27 Nb17 O25 105.5(4) . . ?
O27 Nb17 O29 102.9(4) . . ?
O29 Nb17 Nb21 84.1(3) . . ?
O29 Nb17 Nb23 31.4(3) . . ?
O29 Nb17 O26 154.7(3) . . ?
O29 Nb17 O60 89.7(3) . 2_665 ?
O29 Nb17 O33 79.6(3) . . ?
O29 Nb17 O25 92.8(4) . . ?
Nb12 Nb9 Nb24 62.16(2) . . ?
Nb12 Nb9 Nb2 59.71(3) . . ?
Nb12 Nb9 Nb5 90.76(3) . . ?
Nb24 Nb9 Nb2 90.96(3) . . ?
Nb5 Nb9 Nb24 59.89(3) . . ?
Nb5 Nb9 Nb2 60.22(3) . . ?
O5 Nb9 Nb12 31.48(19) . . ?
O5 Nb9 Nb24 80.6(2) . . ?
O5 Nb9 Nb2 82.0(2) . . ?
O5 Nb9 Nb5 122.13(19) . . ?
O5 Nb9 O16 84.4(3) . . ?
O5 Nb9 O10 76.3(3) . . ?
O16 Nb9 Nb12 81.4(2) . . ?
O16 Nb9 Nb24 32.04(18) . . ?
O16 Nb9 Nb2 122.92(18) . . ?
O16 Nb9 Nb5 82.36(19) . . ?
O16 Nb9 O10 77.2(2) . . ?
O10 Nb9 Nb12 44.95(17) . . ?
O10 Nb9 Nb24 45.30(16) . . ?
O10 Nb9 Nb2 45.68(16) . . ?
O10 Nb9 Nb5 45.82(17) . . ?
O17 Nb9 Nb12 122.9(2) . . ?
O17 Nb9 Nb24 79.4(2) . . ?
O17 Nb9 Nb2 82.0(2) . . ?
O17 Nb9 Nb5 32.1(2) . . ?
O17 Nb9 O5 154.1(3) . . ?
O17 Nb9 O16 87.4(3) . . ?
O17 Nb9 O10 77.9(3) . . ?
O17 Nb9 O19 89.2(4) . . ?
O19 Nb9 Nb12 79.3(2) . . ?
O19 Nb9 Nb24 122.6(2) . . ?
O19 Nb9 Nb2 31.7(2) . . ?
O19 Nb9 Nb5 81.4(2) . . ?
O19 Nb9 O5 87.8(3) . . ?
O19 Nb9 O16 154.5(3) . . ?
O19 Nb9 O10 77.3(3) . . ?
O18 Nb9 Nb12 134.1(3) . . ?
O18 Nb9 Nb24 133.0(3) . . ?
O18 Nb9 Nb2 136.1(3) . . ?
O18 Nb9 Nb5 135.2(3) . . ?
O18 Nb9 O5 102.6(4) . . ?
O18 Nb9 O16 101.0(3) . . ?
O18 Nb9 O10 178.0(4) . . ?
O18 Nb9 O17 103.1(4) . . ?
O18 Nb9 O19 104.4(4) . . ?
Nb16 Nb19 Nb22 59.58(2) . . ?
Nb16 Nb19 Nb13 61.91(3) . . ?
Nb16 Nb19 Nb7 90.04(3) . . ?
Nb13 Nb19 Nb22 91.12(3) . . ?
Nb13 Nb19 Nb7 59.83(3) . . ?
Nb7 Nb19 Nb22 60.04(3) . . ?
O77 Nb19 Nb16 80.1(2) . . ?
O77 Nb19 Nb22 121.86(18) . . ?
O77 Nb19 Nb13 30.87(17) . . ?
O77 Nb19 Nb7 81.95(19) . . ?
O77 Nb19 O70 76.5(2) . . ?
O77 Nb19 O67 83.6(3) . . ?
O70 Nb19 Nb16 43.81(14) . . ?
O70 Nb19 Nb22 45.41(16) . . ?
O70 Nb19 Nb13 45.78(16) . . ?
O70 Nb19 Nb7 46.24(14) . . ?
O67 Nb19 Nb16 31.84(19) . . ?
O67 Nb19 Nb22 81.97(19) . . ?
O67 Nb19 Nb13 80.6(2) . . ?
O67 Nb19 Nb7 121.8(2) . . ?
O67 Nb19 O70 75.6(2) . . ?
O69 Nb19 Nb16 79.2(2) . . ?
O69 Nb19 Nb22 31.3(2) . . ?
O69 Nb19 Nb13 122.4(2) . . ?
O69 Nb19 Nb7 81.0(2) . . ?
O69 Nb19 O77 153.1(3) . . ?
O69 Nb19 O70 76.7(3) . . ?
O69 Nb19 O67 87.8(3) . . ?
O69 Nb19 O79 88.0(3) . . ?
O79 Nb19 Nb16 121.5(2) . . ?
O79 Nb19 Nb22 80.7(2) . . ?
O79 Nb19 Nb13 79.4(2) . . ?
O79 Nb19 Nb7 31.5(2) . . ?
O79 Nb19 O77 88.3(3) . . ?
O79 Nb19 O70 77.7(2) . . ?
O79 Nb19 O67 153.2(3) . . ?
O78 Nb19 Nb16 135.4(3) . . ?
O78 Nb19 Nb22 133.8(3) . . ?
O78 Nb19 Nb13 135.1(3) . . ?
O78 Nb19 Nb7 134.5(3) . . ?
O78 Nb19 O77 104.3(3) . . ?
O78 Nb19 O70 178.9(4) . . ?
O78 Nb19 O67 103.7(4) . . ?
O78 Nb19 O69 102.5(4) . . ?
O78 Nb19 O79 103.0(4) . . ?
Nb18 Nb5 Nb24 61.84(3) . . ?
Nb18 Nb5 Nb2 59.82(3) . . ?
Nb18 Nb5 Nb9 90.57(3) . . ?
Nb24 Nb5 Nb2 90.96(3) . . ?
Nb24 Nb5 Nb9 60.09(3) . . ?
Nb9 Nb5 Nb2 60.02(3) . . ?
O13 Nb5 Nb18 80.2(2) . . ?
O13 Nb5 Nb24 31.4(2) . . ?
O13 Nb5 Nb2 122.2(2) . . ?
O13 Nb5 Nb9 82.5(2) . . ?
O13 Nb5 O10 76.6(3) . . ?
O10 Nb5 Nb18 44.84(15) . . ?
O10 Nb5 Nb24 45.41(16) . . ?
O10 Nb5 Nb2 45.57(16) . . ?
O10 Nb5 Nb9 45.75(15) . . ?
O11 Nb5 Nb18 31.4(2) . . ?
O11 Nb5 Nb24 80.7(2) . . ?
O11 Nb5 Nb2 81.5(2) . . ?
O11 Nb5 Nb9 121.9(2) . . ?
O11 Nb5 O13 84.0(3) . . ?
O11 Nb5 O10 76.1(3) . . ?
O46 Nb5 Nb18 78.9(2) . . ?
O46 Nb5 Nb24 122.5(2) . . ?
O46 Nb5 Nb2 31.6(2) . . ?
O46 Nb5 Nb9 81.7(2) . . ?
O46 Nb5 O13 153.5(3) . . ?
O46 Nb5 O10 77.1(3) . . ?
O46 Nb5 O11 86.5(3) . . ?
O46 Nb5 O17 89.7(3) . . ?
O17 Nb5 Nb18 122.3(2) . . ?
O17 Nb5 Nb24 79.4(2) . . ?
O17 Nb5 Nb2 81.6(3) . . ?
O17 Nb5 Nb9 31.8(2) . . ?
O17 Nb5 O13 87.9(3) . . ?
O17 Nb5 O10 77.5(3) . . ?
O17 Nb5 O11 153.6(3) . . ?
O12 Nb5 Nb18 134.5(3) . . ?
O12 Nb5 Nb24 133.5(3) . . ?
O12 Nb5 Nb2 135.5(3) . . ?
O12 Nb5 Nb9 135.0(3) . . ?
O12 Nb5 O13 102.2(4) . . ?
O12 Nb5 O10 178.7(4) . . ?
O12 Nb5 O11 103.1(4) . . ?
O12 Nb5 O46 104.0(4) . . ?
O12 Nb5 O17 103.2(4) . . ?
Nb26 Nb21 Nb17 61.82(3) . . ?
Nb26 Nb21 Nb11 60.75(4) . . ?
Nb11 Nb21 Nb17 89.34(5) . . ?
O33 Nb21 Nb26 44.47(17) . . ?
O33 Nb21 Nb17 44.85(16) . . ?
O33 Nb21 Nb11 44.66(16) . . ?
O33 Nb21 Nb25 44.19(19) . . ?
O23 Nb21 Nb26 31.0(2) . . ?
O23 Nb21 Nb17 80.0(2) . . ?
O23 Nb21 Nb11 83.5(2) . . ?
O23 Nb21 O33 75.4(3) . . ?
O23 Nb21 Nb25 119.0(2) . . ?
O25 Nb21 Nb26 80.5(2) . . ?
O25 Nb21 Nb17 31.2(2) . . ?
O25 Nb21 Nb11 120.5(2) . . ?
O25 Nb21 O33 75.9(3) . . ?
O25 Nb21 O23 83.9(3) . . ?
O25 Nb21 Nb25 87.9(3) . . ?
O35 Nb21 Nb26 78.6(3) . . ?
O35 Nb21 Nb17 121.5(3) . . ?
O35 Nb21 Nb11 32.3(3) . . ?
O35 Nb21 O33 76.7(3) . . ?
O35 Nb21 O23 87.2(4) . . ?
O35 Nb21 O25 152.5(3) . . ?
O35 Nb21 Nb25 73.8(3) . . ?
O28 Nb21 Nb26 121.3(3) . . ?
O28 Nb21 Nb17 78.6(3) . . ?
O28 Nb21 Nb11 78.6(3) . . ?
O28 Nb21 O33 76.8(3) . . ?
O28 Nb21 O23 152.1(3) . . ?
O28 Nb21 O25 87.0(4) . . ?
O28 Nb21 O35 88.9(4) . . ?
O28 Nb21 Nb25 34.1(3) . . ?
O24 Nb21 Nb26 133.8(4) . . ?
O24 Nb21 Nb17 135.1(4) . . ?
O24 Nb21 Nb11 135.6(4) . . ?
O24 Nb21 O33 178.3(4) . . ?
O24 Nb21 O23 102.9(4) . . ?
O24 Nb21 O25 103.9(4) . . ?
O24 Nb21 O35 103.4(5) . . ?
O24 Nb21 O28 104.8(4) . . ?
O24 Nb21 Nb25 137.5(4) . . ?
Nb25 Nb21 Nb26 88.00(10) . . ?
Nb25 Nb21 Nb17 64.21(11) . . ?
Nb15 Nb11 Nb21 92.37(6) . . ?
Nb15 Nb11 Nb23 61.32(5) . . ?
Nb21 Nb11 Nb23 61.96(6) . . ?
O33 Nb11 Nb15 45.46(18) . . ?
O33 Nb11 Nb21 46.93(18) . . ?
O33 Nb11 Nb23 47.75(18) . . ?
O39 Nb11 Nb15 32.9(2) . . ?
O39 Nb11 Nb21 124.9(2) . . ?
O39 Nb11 Nb23 85.3(3) . . ?
O39 Nb11 O33 78.0(3) . . ?
O39 Nb11 O38 82.9(3) . . ?
O39 Nb11 O35 155.7(3) . . ?
O38 Nb11 Nb15 81.0(2) . . ?
O38 Nb11 Nb21 81.3(2) . . ?
O38 Nb11 Nb23 123.9(2) . . ?
O38 Nb11 O33 76.2(3) . . ?
O35 Nb11 Nb15 124.6(3) . . ?
O35 Nb11 Nb21 32.6(3) . . ?
O35 Nb11 Nb23 85.6(3) . . ?
O35 Nb11 O33 79.2(3) . . ?
O35 Nb11 O38 83.6(4) . . ?
O32 Nb11 Nb15 82.3(3) . . ?
O32 Nb11 Nb21 83.7(3) . . ?
O32 Nb11 Nb23 33.2(3) . . ?
O32 Nb11 O33 80.9(3) . . ?
O32 Nb11 O39 91.5(4) . . ?
O32 Nb11 O38 157.0(4) . . ?
O32 Nb11 O35 93.1(4) . . ?
O36 Nb11 Nb15 133.4(3) . . ?
O36 Nb11 Nb21 134.0(3) . . ?
O36 Nb11 Nb23 137.4(4) . . ?
O36 Nb11 O33 174.8(4) . . ?
O36 Nb11 O39 100.5(4) . . ?
O36 Nb11 O38 98.7(4) . . ?
O36 Nb11 O35 101.4(4) . . ?
O36 Nb11 O32 104.2(5) . . ?
Nb17 Nb23 Nb15 62.09(3) . . ?
Nb17 Nb23 Nb11 90.06(6) . . ?
Nb11 Nb23 Nb15 58.02(6) . . ?
O33 Nb23 Nb15 43.58(17) . . ?
O33 Nb23 Nb17 45.52(16) . . ?
O33 Nb23 Nb11 44.58(16) . . ?
O31 Nb23 Nb15 30.8(2) . . ?
O31 Nb23 Nb17 80.8(2) . . ?
O31 Nb23 Nb11 79.2(3) . . ?
O31 Nb23 O33 74.3(3) . . ?
O31 Nb23 O32 85.5(4) . . ?
O29 Nb23 Nb15 81.4(2) . . ?
O29 Nb23 Nb17 30.9(2) . . ?
O29 Nb23 Nb11 120.9(2) . . ?
O29 Nb23 O33 76.4(3) . . ?
O29 Nb23 O31 86.1(4) . . ?
O29 Nb23 O32 151.3(4) . . ?
O29 Nb23 O28 88.5(4) . . ?
O32 Nb23 Nb15 77.4(3) . . ?
O32 Nb23 Nb17 120.4(3) . . ?
O32 Nb23 Nb11 30.4(3) . . ?
O32 Nb23 O33 74.9(3) . . ?
O28 Nb23 Nb15 118.7(3) . . ?
O28 Nb23 Nb17 79.2(3) . . ?
O28 Nb23 Nb11 77.9(3) . . ?
O28 Nb23 O33 75.2(3) . . ?
O28 Nb23 O31 149.4(3) . . ?
O28 Nb23 O32 85.0(4) . . ?
O30 Nb23 Nb15 137.5(3) . . ?
O30 Nb23 Nb17 138.7(3) . . ?
O30 Nb23 Nb11 131.1(3) . . ?
O30 Nb23 O33 175.4(3) . . ?
O30 Nb23 O31 107.1(4) . . ?
O30 Nb23 O29 108.0(4) . . ?
O30 Nb23 O32 100.7(4) . . ?
O30 Nb23 O28 103.2(4) . . ?
O26 Fe1 O37 76.5(3) 2_665 2_665 ?
O26 Fe1 O60 76.1(3) 2_665 . ?
O60 Fe1 O37 76.1(3) . 2_665 ?
O59 Fe1 O26 162.8(3) . 2_665 ?
O59 Fe1 O37 87.7(3) . 2_665 ?
O59 Fe1 O60 93.7(3) . . ?
O59 Fe1 O62 93.1(3) . . ?
O62 Fe1 O26 94.6(3) . 2_665 ?
O62 Fe1 O37 92.9(3) . 2_665 ?
O62 Fe1 O60 166.9(3) . . ?
O61 Fe1 O26 95.9(3) . 2_665 ?
O61 Fe1 O37 167.3(3) . 2_665 ?
O61 Fe1 O60 92.3(3) . . ?
O61 Fe1 O59 98.3(3) . . ?
O61 Fe1 O62 97.9(3) . . ?
O3 Fe4 Nb12 40.01(16) . 2_665 ?
O3 Fe4 O8 76.8(2) . 2_665 ?
O3 Fe4 O14 76.3(2) . 2_665 ?
O4 Fe4 Nb12 83.1(2) . 2_665 ?
O4 Fe4 O3 94.5(3) . . ?
O4 Fe4 O8 92.7(3) . 2_665 ?
O4 Fe4 O14 167.5(3) . 2_665 ?
O4 Fe4 O1 91.9(3) . . ?
O8 Fe4 Nb12 39.61(16) 2_665 2_665 ?
O14 Fe4 Nb12 84.44(17) 2_665 2_665 ?
O14 Fe4 O8 77.1(3) 2_665 2_665 ?
O1 Fe4 Nb12 127.7(2) . 2_665 ?
O1 Fe4 O3 164.8(3) . . ?
O1 Fe4 O8 89.2(3) . 2_665 ?
O1 Fe4 O14 95.1(3) . 2_665 ?
O2 Fe4 Nb12 138.4(3) . 2_665 ?
O2 Fe4 O3 98.7(3) . . ?
O2 Fe4 O4 99.7(4) . . ?
O2 Fe4 O8 167.2(4) . 2_665 ?
O2 Fe4 O14 90.2(4) . 2_665 ?
O2 Fe4 O1 93.8(4) . . ?
O43 Fe2 O51 76.9(2) . 2_665 ?
O43 Fe2 O41 76.7(3) . . ?
O41 Fe2 O51 76.4(2) . 2_665 ?
O44 Fe2 O43 93.7(3) . . ?
O44 Fe2 O51 92.7(3) . 2_665 ?
O44 Fe2 O41 166.7(3) . . ?
O40 Fe2 O43 163.8(3) . . ?
O40 Fe2 O51 88.0(3) . 2_665 ?
O40 Fe2 O41 94.2(3) . . ?
O40 Fe2 O44 92.9(3) . . ?
O42 Fe2 O43 97.0(5) . . ?
O42 Fe2 O51 169.4(3) . 2_665 ?
O42 Fe2 O41 93.9(4) . . ?
O42 Fe2 O44 96.4(4) . . ?
O42 Fe2 O40 96.9(5) . . ?
O71 Fe3 O64 75.8(2) 2_665 2_665 ?
O68 Fe3 O64 75.9(3) 2_665 2_665 ?
O68 Fe3 O71 77.0(3) 2_665 2_665 ?
O22 Fe3 O64 91.7(3) . 2_665 ?
O22 Fe3 O71 93.2(3) . 2_665 ?
O22 Fe3 O68 165.7(3) . 2_665 ?
O20 Fe3 O64 89.1(3) . 2_665 ?
O20 Fe3 O71 163.7(3) . 2_665 ?
O20 Fe3 O68 93.6(3) . 2_665 ?
O20 Fe3 O22 93.3(3) . . ?
O21 Fe3 O64 167.2(3) . 2_665 ?
O21 Fe3 O71 94.4(3) . 2_665 ?
O21 Fe3 O68 94.1(3) . 2_665 ?
O21 Fe3 O22 97.1(4) . . ?
O21 Fe3 O20 99.6(4) . . ?
Nb26 O26 Nb17 112.0(3) . . ?
Nb26 O26 Fe1 101.0(3) . 2_665 ?
Nb17 O26 Fe1 100.0(3) . 2_665 ?
Nb4 O54 Nb14 89.00(19) . . ?
Nb6 O54 Nb4 88.7(2) . . ?
Nb6 O54 Nb8 93.6(2) . . ?
Nb6 O54 Nb10 94.5(2) . . ?
Nb6 O54 Nb14 176.8(3) . . ?
Nb6 O54 Nb20 89.7(2) . . ?
Nb8 O54 Nb4 88.9(2) . . ?
Nb8 O54 Nb10 93.3(2) . . ?
Nb8 O54 Nb14 88.50(19) . . ?
Nb8 O54 Nb20 175.8(3) . . ?
Nb10 O54 Nb4 176.1(3) . . ?
Nb10 O54 Nb14 87.8(2) . . ?
Nb10 O54 Nb20 89.0(2) . . ?
Nb20 O54 Nb4 88.7(2) . . ?
Nb20 O54 Nb14 88.06(19) . . ?
Nb10 O43 Nb6 112.4(3) 2_665 2_665 ?
Fe2 O43 Nb6 99.9(3) . 2_665 ?
Fe2 O43 Nb10 100.0(3) . 2_665 ?
Nb6 O51 Nb8 112.0(3) . . ?
Nb6 O51 Fe2 99.5(2) . 2_665 ?
Nb8 O51 Fe2 99.5(3) . 2_665 ?
Nb1 O64 Fe3 98.8(3) . 2_665 ?
Nb16 O64 Nb1 111.2(3) . . ?
Nb16 O64 Fe3 98.8(3) . 2_665 ?
Nb8 O53 Nb4 114.7(3) . . ?
Nb1 O63 Nb22 114.3(3) . . ?
Nb12 O3 Nb24 112.7(3) 2_665 2_665 ?
Nb12 O3 Fe4 99.8(3) 2_665 . ?
Nb24 O3 Fe4 100.5(3) 2_665 . ?
Nb20 O50 Nb4 115.4(3) . . ?
Nb26 O37 Fe1 98.8(3) . 2_665 ?
Nb15 O37 Nb26 110.4(3) . . ?
Nb15 O37 Fe1 99.4(3) . 2_665 ?
Nb12 O4 Fe4 166.3(4) . . ?
Nb1 O73 Nb7 117.0(3) . . ?
Nb20 O75 Nb14 116.4(3) . . ?
Nb15 O60 Fe1 100.4(3) 2_665 . ?
Nb17 O60 Nb15 112.9(3) 2_665 2_665 ?
Nb17 O60 Fe1 100.0(3) 2_665 . ?
Nb12 O8 Nb18 112.1(3) . . ?
Nb12 O8 Fe4 98.6(2) . 2_665 ?
Nb18 O8 Fe4 98.9(3) . 2_665 ?
Nb1 O71 Nb13 112.5(3) . . ?
Nb1 O71 Fe3 101.2(3) . 2_665 ?
Nb13 O71 Fe3 99.6(3) . 2_665 ?
Nb8 O58 Nb14 114.3(3) . . ?
Nb8 O41 Fe2 100.3(3) 2_665 . ?
Nb10 O41 Nb8 112.9(3) 2_665 2_665 ?
Nb10 O41 Fe2 100.1(3) 2_665 . ?
Nb6 O47 Nb4 114.5(3) . . ?
Nb4 O80 Nb14 116.5(3) . . ?
Nb8 O59 Fe1 157.4(5) . . ?
Nb12 O6 Nb2 114.4(3) . . ?
Nb6 O45 Nb20 115.7(3) . . ?
Nb16 O68 Nb13 111.1(3) . . ?
Fe3 O68 Nb16 101.8(3) 2_665 . ?
Fe3 O68 Nb13 99.8(3) 2_665 . ?
Nb10 O56 Nb14 115.7(3) . . ?
Nb10 O49 Nb20 115.3(3) . . ?
Nb12 O5 Nb9 115.8(3) . . ?
Nb12 O5 Li5 118.9(4) . . ?
Nb9 O5 Li5 120.7(4) . . ?
Nb18 O14 Fe4 99.2(3) . 2_665 ?
Nb24 O14 Nb18 111.9(3) . . ?
Nb24 O14 Fe4 99.8(3) . 2_665 ?
Nb16 O66 Nb22 115.1(3) . . ?
Nb24 O13 Nb5 115.1(4) . . ?
Nb13 O34 Nb7 115.2(3) . . ?
Nb22 O72 Nb7 116.5(3) . . ?
Nb24 O16 Nb9 114.4(3) . . ?
Nb6 O44 Fe2 163.8(4) . . ?
Nb12 O10 Nb24 93.5(2) . . ?
Nb12 O10 Nb2 88.8(2) . . ?
Nb12 O10 Nb9 89.3(2) . . ?
Nb12 O10 Nb5 176.8(3) . . ?
Nb18 O10 Nb12 93.2(2) . . ?
Nb18 O10 Nb24 92.9(2) . . ?
Nb18 O10 Nb2 89.3(2) . . ?
Nb18 O10 Nb9 176.8(3) . . ?
Nb18 O10 Nb5 89.1(2) . . ?
Nb24 O10 Nb2 176.7(3) . . ?
Nb24 O10 Nb9 89.0(2) . . ?
Nb24 O10 Nb5 88.7(2) . . ?
Nb9 O10 Nb2 88.7(2) . . ?
Nb9 O10 Nb5 88.4(2) . . ?
Nb5 O10 Nb2 88.9(2) . . ?
Nb18 O11 Nb5 115.4(3) . . ?
Nb1 O62 Fe1 173.2(4) . . ?
Nb13 O77 Nb19 116.4(3) . . ?
Nb15 O40 Fe2 156.1(5) . . ?
Nb26 O33 Nb17 93.9(2) . . ?
Nb26 O33 Nb21 88.6(2) . . ?
Nb26 O33 Nb11 92.2(3) . . ?
Nb26 O33 Nb23 177.4(4) . . ?
Nb15 O33 Nb26 93.6(3) . . ?
Nb15 O33 Nb17 94.5(3) . . ?
Nb15 O33 Nb21 176.2(3) . . ?
Nb15 O33 Nb11 88.3(2) . . ?
Nb15 O33 Nb23 89.0(3) . . ?
Nb17 O33 Nb21 88.5(2) . . ?
Nb17 O33 Nb23 86.1(2) . . ?
Nb21 O33 Nb23 88.8(2) . . ?
Nb11 O33 Nb17 173.1(3) . . ?
Nb11 O33 Nb21 88.4(3) . . ?
Nb11 O33 Nb23 87.7(2) . . ?
Nb25 O33 Nb26 165.9(4) . . ?
Nb25 O33 Nb15 92.3(3) . . ?
Nb25 O33 Nb17 98.4(3) . . ?
Nb25 O33 Nb21 84.9(3) . . ?
Nb1 O70 Nb22 90.2(2) . . ?
Nb1 O70 Nb13 93.6(2) . . ?
Nb1 O70 Nb7 89.4(2) . . ?
Nb1 O70 Nb19 176.6(3) . . ?
Nb16 O70 Nb1 93.4(2) . . ?
Nb16 O70 Nb22 90.0(2) . . ?
Nb16 O70 Nb13 93.7(2) . . ?
Nb16 O70 Nb7 176.8(3) . . ?
Nb16 O70 Nb19 89.6(2) . . ?
Nb22 O70 Nb13 174.6(3) . . ?
Nb22 O70 Nb7 88.4(2) . . ?
Nb22 O70 Nb19 88.3(2) . . ?
Nb13 O70 Nb7 87.7(2) . . ?
Nb13 O70 Nb19 87.8(2) . . ?
Nb7 O70 Nb19 87.48(19) . . ?
Nb26 O23 Nb21 116.1(4) . . ?
Nb16 O1 Fe4 157.3(5) . . ?
Nb16 O67 Nb19 114.8(3) . . ?
Nb18 O9 Nb2 114.8(3) . . ?
Nb22 O69 Nb19 117.0(4) . . ?
Nb22 O69 Li1 123.1(5) . . ?
Nb19 O69 Li1 119.3(5) . . ?
Nb20 O48 Li16 132.5(7) . 8_756 ?
Nb5 O46 Nb2 117.0(4) . . ?
Nb10 O55 Li20 143.2(5) . 4_566 ?
Nb9 O17 Nb5 116.1(4) . . ?
Nb15 O39 Nb11 113.4(4) . . ?
Nb15 O39 Nb3 120.5(4) . . ?
Nb26 O22 Fe3 171.1(4) . . ?
Nb18 O20 Fe3 159.4(5) . . ?
Nb7 O79 Nb19 116.4(3) . . ?
Nb17 O25 Nb21 116.4(4) . . ?
Nb26 O38 Nb11 112.3(4) . . ?
Nb3 O38 Nb26 124.4(5) . . ?
Nb2 O19 Nb9 116.5(3) . . ?
Nb15 O31 Nb23 116.8(4) . . ?
Nb15 O31 Nb25 105.8(4) . . ?
Nb17 O29 Nb23 117.7(5) . . ?
Nb17 O29 Nb25 106.7(4) . . ?
Nb11 O35 Nb21 115.1(5) . . ?
Nb3 O35 Nb21 124.1(5) . . ?
Nb11 O32 Nb23 116.5(4) . . ?
Nb25 O32 Nb3 112.0(5) . . ?
Fe4 O2 Li5 119.0(5) . . ?
Nb21 O28 Nb23 119.2(4) . . ?
Nb25 O28 Nb21 109.5(4) . . ?
Nb26 Nb3 Nb25 86.28(14) . . ?
O39 Nb3 Nb26 80.8(2) . . ?
O39 Nb3 O32 73.2(4) . . ?
O39 Nb3 Nb25 71.7(3) . . ?
O38 Nb3 Nb26 29.8(3) . . ?
O38 Nb3 O39 87.4(4) . . ?
O38 Nb3 O35 95.6(5) . . ?
O38 Nb3 O32 140.0(4) . . ?
O38 Nb3 Nb25 115.9(3) . . ?
O35 Nb3 Nb26 81.4(3) . . ?
O35 Nb3 O39 137.7(5) . . ?
O35 Nb3 O32 78.0(5) . . ?
O35 Nb3 Nb25 69.1(4) . . ?
O32 Nb3 Nb26 111.0(3) . . ?
O32 Nb3 Nb25 25.0(2) . . ?
O36 Nb3 Nb26 158.0(6) . . ?
O36 Nb3 O39 100.0(5) . . ?
O36 Nb3 O38 128.3(7) . . ?
O36 Nb3 O35 110.5(5) . . ?
O36 Nb3 O32 90.0(6) . . ?
O36 Nb3 Nb25 115.0(6) . . ?
Nb15 Nb25 Nb3 65.35(13) . . ?
Nb21 Nb25 Nb15 96.28(14) . . ?
Nb21 Nb25 Nb3 65.12(14) . . ?
O33 Nb25 Nb15 45.4(2) . . ?
O33 Nb25 Nb21 50.9(2) . . ?
O33 Nb25 O29 74.5(3) . . ?
O33 Nb25 Nb3 52.6(2) . . ?
O31 Nb25 Nb15 34.8(2) . . ?
O31 Nb25 Nb21 128.2(3) . . ?
O31 Nb25 O33 78.3(3) . . ?
O31 Nb25 O29 73.5(4) . . ?
O31 Nb25 Nb3 93.8(3) . . ?
O29 Nb25 Nb15 78.6(2) . . ?
O29 Nb25 Nb21 82.9(3) . . ?
O29 Nb25 Nb3 127.1(3) . . ?
O32 Nb25 Nb15 87.6(4) . . ?
O32 Nb25 Nb21 97.3(5) . . ?
O32 Nb25 O33 94.8(5) . . ?
O32 Nb25 O31 96.0(5) . . ?
O32 Nb25 O29 166.1(5) . . ?
O32 Nb25 O28 107.8(6) . . ?
O32 Nb25 O30 106.2(5) . . ?
O32 Nb25 Nb3 43.0(4) . . ?
O28 Nb25 Nb15 130.3(3) . . ?
O28 Nb25 Nb21 36.4(3) . . ?
O28 Nb25 O33 85.6(4) . . ?
O28 Nb25 O31 152.3(5) . . ?
O28 Nb25 O29 80.6(5) . . ?
O28 Nb25 O30 95.9(4) . . ?
O28 Nb25 Nb3 94.0(4) . . ?
O30 Nb25 Nb15 125.6(3) . . ?
O30 Nb25 Nb21 131.9(3) . . ?
O30 Nb25 O33 157.4(4) . . ?
O30 Nb25 O31 90.9(4) . . ?
O30 Nb25 O29 83.4(4) . . ?
O30 Nb25 Nb3 149.1(3) . . ?
O69 Li1 Li8 132.4(7) . . ?
Li7 Li4 Li21 63.2(7) . . ?
O93 Li6 Li3 103.1(8) . 3_646 ?
O93 Li6 Li9 96.3(7) . . ?
Li9 Li6 Li3 66.1(7) . 3_646 ?
Li7 Li12 Li12 58.5(6) 2_665 2_665 ?
Li7 Li12 Li12 56.2(6) . 2_665 ?
Li7 Li12 Li7 58.2(10) 2_665 . ?
Li22 Li14 Li10 101.5(9) . . ?
O48 Li16 Li13 101.7(6) 8_755 5_766 ?
O48 Li16 Li2 82.7(6) 8_755 8_755 ?
Li2 Li16 Li13 63.9(5) 8_755 5_766 ?
O55 Li20 Li18 97.6(7) 4_466 3_646 ?
Li21 Li22 Li14 136.0(14) . . ?
Li23 Li3 Li6 103.5(9) 2_565 3_656 ?
O105 Li13 Li16 88.8(8) 4_566 5_766 ?
O105 Li13 Li11 108.3(10) 4_566 . ?
Li11 Li13 Li16 154.5(7) . 5_766 ?
Li4 Li7 Li12 133.7(9) . 2_665 ?
Li4 Li7 Li12 160.6(10) . . ?
Li4 Li7 Li7 121.2(7) . 2_665 ?
Li4 Li7 Li21 63.5(8) . . ?
Li12 Li7 Li12 65.3(9) 2_665 . ?
Li12 Li7 Li21 115.5(10) 2_665 . ?
Li12 Li7 Li21 115.8(8) . . ?
Li7 Li7 Li12 59.6(8) 2_665 . ?
Li7 Li7 Li12 62.2(6) 2_665 2_665 ?
Li7 Li7 Li21 175.2(6) 2_665 . ?
Li5 Li2 Li16 91.4(6) 8_756 8_756 ?
O5 Li5 Li2 146.0(5) . 8_755 ?
O2 Li5 O5 101.6(4) . . ?
O2 Li5 Li2 89.9(5) . 8_755 ?
Li22 Li21 Li4 74.3(8) . . ?
Li22 Li21 Li7 127.0(9) . . ?
Li7 Li21 Li4 53.2(6) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Nb4 Nb6 O44 Fe2 123.0(15) . . . . ?
Nb4 Nb8 O59 Fe1 -125.3(9) . . . . ?
Nb4 Nb20 O48 Li16 163.4(5) . . . 8_756 ?
Nb6 Nb20 O48 Li16 -108.7(7) . . . 8_756 ?
Nb10 Nb20 O48 Li16 -17.1(8) . . . 8_756 ?
Nb14 Nb8 O59 Fe1 -33.9(11) . . . . ?
Nb14 Nb10 O55 Li20 44.3(13) . . . 4_566 ?
Nb14 Nb20 O48 Li16 71.5(7) . . . 8_756 ?
Nb20 Nb6 O44 Fe2 32.1(18) . . . . ?
Nb20 Nb10 O55 Li20 139.1(10) . . . 4_566 ?
Nb22 Nb16 O1 Fe4 -123.2(11) . . . . ?
Nb26 O38 Nb3 O39 -75.9(6) . . . . ?
Nb26 O38 Nb3 O35 61.8(6) . . . . ?
Nb26 O38 Nb3 O32 -16.2(11) . . . . ?
Nb26 O38 Nb3 O36 -176.6(6) . . . . ?
Nb26 O38 Nb3 Nb25 -7.7(7) . . . . ?
Nb15 Nb11 O32 Nb23 47.3(5) . . . . ?
Nb2 Nb12 O4 Fe4 120.3(16) . . . . ?
Nb2 Nb18 O20 Fe3 -125.6(12) . . . . ?
Nb9 Nb12 O4 Fe4 29.6(19) . . . . ?
Nb19 Nb16 O1 Fe4 -32.6(14) . . . . ?
Nb5 Nb18 O20 Fe3 -33.6(15) . . . . ?
Nb21 Nb11 O32 Nb23 -45.9(5) . . . . ?
Nb21 O28 Nb25 Nb15 24.6(9) . . . . ?
Nb21 O28 Nb25 O33 15.8(5) . . . . ?
Nb21 O28 Nb25 O31 70.0(13) . . . . ?
Nb21 O28 Nb25 O29 90.8(5) . . . . ?
Nb21 O28 Nb25 O32 -77.8(7) . . . . ?
Nb21 O28 Nb25 O30 173.1(5) . . . . ?
Nb21 O28 Nb25 Nb3 -36.2(5) . . . . ?
Nb11 Nb15 O40 Fe2 -118.9(9) . . . . ?
Nb23 Nb15 O40 Fe2 -29.3(12) . . . . ?
Fe4 Nb12 O4 Fe4 -101.5(17) 2_665 . . . ?
O43 Nb6 O44 Fe2 -59.8(16) 2_665 . . . ?
O43 Nb10 O55 Li20 -127.5(11) 2_665 . . 4_566 ?
O51 Nb6 O44 Fe2 -139.9(16) . . . . ?
O51 Nb8 O59 Fe1 140.2(9) . . . . ?
O64 Nb16 O1 Fe4 141.0(12) . . . . ?
O53 Nb8 O59 Fe1 -127.3(10) . . . . ?
O3 Nb12 O4 Fe4 -61.5(17) 2_665 . . . ?
O50 Nb20 O48 Li16 163.4(6) . . . 8_756 ?
O37 Nb15 O40 Fe2 142.3(10) . . . . ?
O75 Nb20 O48 Li16 70.8(7) . . . 8_756 ?
O60 Nb15 O40 Fe2 61.4(10) 2_665 . . . ?
O8 Nb12 O4 Fe4 -142.4(16) . . . . ?
O8 Nb18 O20 Fe3 140.0(13) . . . . ?
O58 Nb8 O59 Fe1 -31.0(10) . . . . ?
O41 Nb8 O59 Fe1 59.7(10) 2_665 . . . ?
O41 Nb10 O55 Li20 -48.7(11) 2_665 . . 4_566 ?
O47 Nb6 O44 Fe2 125.7(16) . . . . ?
O6 Nb12 O4 Fe4 123.6(17) . . . . ?
O45 Nb6 O44 Fe2 31.3(17) . . . . ?
O45 Nb20 O48 Li16 -106.3(7) . . . 8_756 ?
O68 Nb16 O1 Fe4 60.5(12) . . . . ?
O56 Nb10 O55 Li20 43.7(12) . . . 4_566 ?
O49 Nb10 O55 Li20 140.5(11) . . . 4_566 ?
O49 Nb20 O48 Li16 -19.5(7) . . . 8_756 ?
O5 Nb12 O4 Fe4 29.3(17) . . . . ?
O14 Nb18 O20 Fe3 58.6(13) . . . . ?
O66 Nb16 O1 Fe4 -125.4(12) . . . . ?
O11 Nb18 O20 Fe3 -33.4(14) . . . . ?
O33 Nb11 O32 Nb23 1.4(5) . . . . ?
O67 Nb16 O1 Fe4 -31.1(12) . . . . ?
O9 Nb18 O20 Fe3 -127.8(13) . . . . ?
O39 Nb15 O40 Fe2 -124.4(10) . . . . ?
O39 Nb11 O32 Nb23 79.0(5) . . . . ?
O38 Nb11 O32 Nb23 3.6(14) . . . . ?
O31 Nb15 O40 Fe2 -28.6(11) . . . . ?
O35 Nb11 O32 Nb23 -77.2(5) . . . . ?
O36 Nb11 O32 Nb23 -179.8(5) . . . . ?
Nb3 O32 Nb25 Nb15 -55.4(5) . . . . ?
Nb3 O32 Nb25 Nb21 40.6(5) . . . . ?
Nb3 O32 Nb25 O33 -10.5(6) . . . . ?
Nb3 O32 Nb25 O31 -89.2(5) . . . . ?
Nb3 O32 Nb25 O29 -49(3) . . . . ?
Nb3 O32 Nb25 O28 76.4(6) . . . . ?
Nb3 O32 Nb25 O30 178.2(4) . . . . ?
Nb25 Nb15 O40 Fe2 -41.7(12) . . . . ?

loop_
_platon_missing_refln_index_h
_platon_missing_refln_index_k
_platon_missing_refln_index_l
_platon_missing_refln_theta
1 1 0 2.385
0 2 0 2.726
0 8 0 10.967
2 10 0 14.325
1 1 1 2.593
2 1 1 4.271
3 3 1 7.244
5 4 1 11.319
6 11 1 19.436
2 12 1 17.095
6 12 1 20.595
0 0 2 2.034
1 0 2 2.823
7 0 2 13.986
0 1 2 2.449
1 1 2 3.136
0 2 2 3.402
2 3 2 6.024
7 6 2 16.300
6 7 2 15.449
7 9 2 18.834
2 11 2 15.823
1 14 2 19.666
4 3 3 9.384
1 0 4 4.518
4 0 4 8.856
3 3 4 8.257
3 4 4 9.021
2 5 4 8.883
7 6 4 16.697
5 8 4 15.385
8 8 5 20.154
5 0 6 11.610
2 3 6 8.351
1 4 6 8.442
4 4 6 11.397
2 1 7 8.265
2 3 7 9.132
10 5 7 22.481
0 0 8 8.163
2 2 8 9.473
7 3 8 16.682
2 4 8 10.605
9 7 8 22.166
1 3 9 10.267
4 3 9 12.824
0 11 10 18.428
3 5 11 14.507
3 8 11 16.930
1 1 12 12.533
2 3 12 13.578
3 3 13 15.209
4 3 13 16.109
4 7 13 18.397
2 1 14 14.998
2 7 15 18.743
6 1 17 21.438
2 2 19 20.324

_platon_squeeze_details          
;
TITL shelx            P c c n      R = 0.09
CELL   22.5729   32.4190   43.4373     90.00     90.00     90.00
SPGR Pccn
# Solvent Accessible Volume =      8196
# Electrons Found in S.A.V. =      1996
# Note: Atoms in Void are Labelled as Cxxx and Qxxx for all Others
C101 0.352 0.805 0.072 !       4.39 eA-3
C102 0.930 0.572 0.090 !       3.57 eA-3
Q103 0.929 0.990 0.294 !       3.41 eA-3
Q104 0.102 0.846 0.046 !       3.35 eA-3
C105 0.123 0.884 0.326 !       2.98 eA-3
Q106 0.290 0.284 0.794 !       2.92 eA-3
Q107 0.714 0.291 0.257 !       2.92 eA-3
Q108 0.024 0.350 0.598 !       2.83 eA-3
Q109 0.718 0.572 0.480 !       2.81 eA-3
Q110 0.021 0.007 0.171 !       2.78 eA-3
Q111 0.155 0.562 0.183 !       2.76 eA-3
Q112 0.413 0.833 0.270 !       2.64 eA-3
C113 0.141 0.470 0.120 !       2.57 eA-3
Q114 0.118 0.954 0.139 !       2.52 eA-3
Q115 0.401 0.531 0.389 !       2.49 eA-3
Q116 0.734 0.696 0.428 !       2.42 eA-3
Q117 0.194 0.991 0.301 !       2.42 eA-3
Q118 0.580 0.525 0.285 !       2.35 eA-3
Q119 0.357 0.694 0.175 !       2.30 eA-3
Q120 0.177 0.242 0.115 !       2.29 eA-3
Q121 0.250 0.254 0.406 !       2.24 eA-3
C122 0.399 0.876 0.002 !       2.21 eA-3
Q123 0.093 0.591 0.247 !       2.20 eA-3
Q124 0.556 0.367 0.147 !       2.19 eA-3
Q125 0.460 0.204 0.277 !       2.16 eA-3
Q126 0.563 0.328 0.069 !       2.14 eA-3
Q127 0.147 0.073 0.024 !       2.10 eA-3
C128 0.445 0.584 0.448 !       2.09 eA-3
Q129 0.405 0.039 0.154 !       2.06 eA-3
C130 0.113 0.654 0.942 !       2.05 eA-3
Q131 0.744 0.368 0.123 !       2.04 eA-3
C132 0.633 0.578 0.431 !       1.93 eA-3
Q133 0.130 0.092 0.582 !       1.88 eA-3
Q134 0.992 0.679 0.833 !       1.87 eA-3
Q135 0.687 0.779 0.169 !       1.86 eA-3
C136 0.314 0.700 0.097 !       1.86 eA-3
Q137 0.538 0.233 0.168 !       1.82 eA-3
Q138 0.837 0.385 0.539 !       1.79 eA-3
C139 0.774 0.032 0.392 !       1.79 eA-3
Q140 0.229 0.256 0.285 !       1.76 eA-3
Q141 0.624 0.969 0.757 !       1.75 eA-3
Q142 0.976 0.094 0.014 !       1.74 eA-3
Q143 0.485 0.054 0.139 !       1.71 eA-3
Q144 0.541 0.446 0.325 !       1.64 eA-3
Q145 0.305 0.995 0.031 !       1.63 eA-3
Q146 0.698 0.633 0.442 !       1.60 eA-3
C147 0.220 0.897 0.486 !       1.60 eA-3
Q148 0.704 0.092 0.029 !       1.59 eA-3
Q149 0.609 0.302 0.906 !       1.58 eA-3
Q150 0.617 0.790 0.208 !       1.57 eA-3
Q151 0.495 0.665 0.153 !       1.55 eA-3
Q152 0.209 0.704 0.522 !       1.54 eA-3
Q153 0.165 0.625 0.443 !       1.52 eA-3
Q154 0.361 0.319 0.877 !       1.51 eA-3
Q155 0.139 0.222 0.286 !       1.49 eA-3
Q156 0.264 0.604 0.255 !       1.47 eA-3
Q157 0.227 0.350 0.045 !       1.45 eA-3
Q158 0.727 0.650 0.455 !       1.45 eA-3
Q159 0.765 0.934 0.903 !       1.45 eA-3
C160 0.706 0.194 0.014 !       1.44 eA-3
Q161 0.475 0.837 0.246 !       1.44 eA-3
Q162 0.066 0.633 0.717 !       1.44 eA-3
Q163 0.990 0.116 0.295 !       1.42 eA-3
C164 0.484 0.945 0.149 !       1.41 eA-3
Q165 0.487 0.765 0.328 !       1.41 eA-3
Q166 0.032 0.678 0.846 !       1.40 eA-3
C167 0.195 0.680 0.509 !       1.40 eA-3
Q168 0.296 0.875 0.139 !       1.40 eA-3
C169 0.827 0.283 0.555 !       1.40 eA-3
Q170 0.080 0.726 0.596 !       1.40 eA-3
Q171 0.678 0.414 0.191 !       1.38 eA-3
C172 0.115 0.704 0.336 !       1.37 eA-3
Q173 0.470 0.478 0.262 !       1.37 eA-3
Q174 0.531 0.030 0.197 !       1.36 eA-3
Q175 0.094 0.289 0.185 !       1.36 eA-3
Q176 0.617 0.643 0.658 !       1.35 eA-3
Q177 0.227 0.922 0.740 !       1.33 eA-3
C178 0.405 0.835 0.878 !       1.33 eA-3
Q179 0.204 0.088 0.495 !       1.33 eA-3
C180 0.501 0.335 0.119 !       1.33 eA-3
Q181 0.499 0.782 0.314 !       1.30 eA-3
Q182 0.416 0.720 0.922 !       1.30 eA-3
C183 0.749 0.115 0.382 !       1.30 eA-3
Q184 0.641 0.171 0.706 !       1.29 eA-3
Q185 0.236 0.446 0.902 !       1.29 eA-3
Q186 0.665 0.492 0.872 !       1.26 eA-3
Q187 0.983 0.721 0.300 !       1.26 eA-3
Q188 0.565 0.454 0.995 !       1.25 eA-3
Q189 0.210 0.290 0.416 !       1.25 eA-3
Q190 0.323 0.299 0.882 !       1.25 eA-3
Q191 0.797 0.771 0.104 !       1.24 eA-3
C192 0.570 0.423 0.427 !       1.23 eA-3
Q193 0.829 0.490 0.728 !       1.23 eA-3
Q194 0.881 0.202 0.392 !       1.23 eA-3
Q195 0.169 0.296 0.493 !       1.22 eA-3
Q196 0.533 0.797 0.295 !       1.22 eA-3
Q197 0.501 0.273 0.119 !       1.21 eA-3
Q198 0.890 0.007 0.544 !       1.19 eA-3
Q199 0.166 0.334 0.857 !       1.19 eA-3
;
_platon_squeeze_special_details  ?
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.431 -0.069 0.000 4062 982 ' '
2 0.963 0.037 0.500 4062 982 ' '
3 0.250 0.250 0.286 19 8 ' '
4 0.250 0.250 0.786 19 8 ' '
5 0.750 0.750 0.214 20 8 ' '
6 0.750 0.750 0.714 20 8 ' '

_platon_squeeze_void_probe_radius 1.20

_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details 
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 59.988
_oxdiff_exptl_absorpt_empirical_full_min 0.413
_exptl_crystal_recrystallization_method 'Re-crystallisation from solvent: Water'
